The Science and Engineering of Granulation Processes
Libro dedicado a la granulación...
The Science and Engineering of Granulation Processes
Particle Technology Series Series Editor Professor Brian Scarlett Technical University of Delft
The Kluwer Particle Technology Series of books is the successor to the Chapman and Hall Powder Technology Series. The aims are the same, the scope is wider. The particles involved may be solid or they may be droplets. The size range may be granular, powder or nano-scale. The accent may be on materials or on equipment, it may be practical or theoretical. Each book can add one brick to a fascinating and vital technology. Such a vast field cannot be covered by a carefully organised tome or encyclopaedia. Any author who has a view or experience to contribute is welcome. The subject of particle technology is set to enjoy its golden times at the start of the new millennium and I expect that the growth of this series of books will reflect that trend.
The Science and Engineering of Granulation Processes JIM LITSTER The University of Queensland, Brisbane, Australia
BRYAN ENNIS E&G Associates, Nashville, Tennessee, U.S.A.
LIAN LIU (Associate Editor) The University of Queensland, Brisbane, Australia
SPRINGER-SCIENCE+BUSINESS MEDIA, B.V.
A C.I.P. Catalogue record for this book is available from the Library of Congress.
ISBN 978-90-481-6533-9 ISBN 978-94-017-0546-2 (eBook) DOI 10.1007/978-94-017-0546-2
Printed on acid-free paper
All Rights Reserved © 2004 Springer Science+Business Media Dordrecht Originally published by Kluwer Academic Publishers in 2004 Softcover reprint ofthe hardcover 1st edition No part of this work may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, microfilming, recording or otherwise, without written permission from the Publisher, with the exception of any material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work.
Dedication To my wife, Annette, and my children, Sam, Rachel and Angus, for their unfailing love and support.
Preface This book had its origins in a meeting between two (relatively) young particle technology researchers on Rehobeth Beach in Delaware in 1992 near the holiday house of Reg Davies (then Director of the Particle Science and Technology Research Center in Dupont). As we played in the sand, we shared an excitement for developments in particle technology, especially particle characterization, that would lead operations such as granulation to be placed on a sound scientific and engineering footing. The immediate outcome from this interaction was the development of new industry short courses in granulation and related topics which we taught together both in Australia and North America. This book follows closely the structure and approaches developed in these courses, particularly the emphasis on particle design in granulation, where the impact of both formulation properties and process variables on product attributes needs to be understood and quantified. The book has been a long time in the making. We have been actively preparing the book for at least five years. Although the chapters have relatively good bibliographies, this book is not a review of the field. Rather it is an attempt by the authors to present a comprehensive engineering approach to granulator design, scale up and operation. It is exciting for us to see the explosion of research interest around the world in this area in the last five to seven years. Some of the most recent work will have to find its way into the second edition. The book is written primarily as a tool for engineers and technologists in industrial R&D to use directly in the engineering design and troubleshooting. It should also be a useful text or reference for honours and graduate student level courses in Particle Technology. Indeed, drafts of some chapters have already been tested on students in Chemical Engineering at the Universities of Queensland and Delaware. Chapter 1 gives a good overview of the approach taken and advice for readers on how to make best use of the book. The book relies heavily on work of current and former research students at The University of Queensland and we owe a great debt of gratitude to these people – Anthony Adetayo, Lian Liu, Rakhman Sarwono, Simon Iveson, Karen Hapgood, Hans Wildeboer and Rachel Smith. We also want acknowledge a wide range of research colleagues from industry and academia who have contributed strongly in the research development through discussion and active collaborations: Ian Cameron, Ted White, Tony Howes and Fu Yang Wang (University of Queensland), Neil Page, Simon Iveson and Simon Biggs (University of Newcastle), Flip Wauters, Gabrie Meesters and Brian Scarlett (Delft Technical University) Jim Michaels (Merck and Co), Paul Mort (P&G), Greg Sunshine (Dupont), Gabriel Tardos (City College, New York), Mike Hounslow (Cambridge and Sheffield Universities), Sarah Forrest and John Bridgwater (Cambridge University), Jonathan Seville (Surrey and Birmingham Universities). JL would particularly like to thank Lian Liu (Research Fellow) for her constructive criticisms of the manuscript and enormous assistance in editorial work and Vicki Thompson, without whose dedicated efforts in preparation of the manuscript this book would never have seen the light of day.
Jim Litster Bryan Ennis September 2003
CONTENTS Preface 1
1.1 1.2 1.3 1.4
4 6 8 9
Granulation Rate Processes Considering a Granulator as a Reactor Granulation as Particle Design How To Use This Book
Particle and Granule Morphology 2.1 Particle Size, Shape and Size Distribution 2.1.1 Particle Size Definitions 2.1.2 Particle Shape 2.1.3 Basic Particle Size Distribution Definitions 2.1.4 Different Ways to Represent Particle Size Distributions 2.1.5 Measures of Mean Size and Spread of the Size Distribution 2.1.6 Particle Size Measurement 2.1.7 Particle Size Summary 2.2 Density, Porosity and Pore Size Distribution 2.2.1 Density and Porosity Definitions 2.2.2 Density Measurement 2.2.3 Porosity and Pore Size Distribution Measurement 2.3 Granule Properties 2.3.1 Granule Size Distribution 2.3.2 Porosity and Granule Density 2.3.3 Wet Granule Morphology 2.3.4 Granule Performance Properties 2.4 Summary 2.5 Bibliography 2.6 Nomenclature
12 12 13 17 20 22 23 24 25 25 27 28 29 30 31 32 32 34 34 35
Wetting, Nucleation and Binder Distribution 3.1 Powder Surface Properties 3.1.1 Some Definitions 3.1.2 Methods of Measurement 3.2 Wetting and Nucleation Regimes for Granulation 3.2.1 Drop Penetration into Powder Beds 3.2.2 Analysis of the Spray Zone in Granulators – the Dimensionless Spray Flux 3.2.3 A Nucleation Regime Map 3.2.4 Related Studies on Wetting and Nucleation 3.3 Control of Wetting and Nucleation for Particle Design ix
40 40 43 52 53 59 63 65 68
x 3.3.1 Adhesion Tension Control 3.3.2 Other Powder and Liquid Properties 3.3.3 Spray Distribution 3.3.4 Agitation Intensity 3.3.5 Simultaneous Drying 3.3.6 Concluding Comments 3.4 Bibliography 4
Consolidation, Coalescence and Growth 4.1 Granule Mechanics 4.1.1 Measuring the Dynamic Yield Stress of a Particle Assembly 4.2 Granule Consolidation 4.2.1 A Mechanistic Understanding of Granulation 4.2.2 Effect of Formulation Properties and Process Conditions on Consolidation 4.2.3 Granule Consolidation with Simultaneous Drying 4.2.4 Theoretical Models for Consolidation 4.3 Granule Coalescence Criteria for Near Elastic Particles 4.3.1 Growth Regimes for near Elastic Granules 4.3.2 Estimating the Characteristic Collision Velocity 4.3.3 Examples of Application of the Stokes Regime Analysis 4.3.4 Limitations of the Stokes Regime Analysis and Final Remarks 4.4 Granule Coalescence Criteria for Deformable, Porous Granules 4.4.1 Development of Coalescence Criteria 4.4.2 Implications of the Coalescence Criteria 4.4.3 Extension to Surface Dry Granules 4.4.4 Comparison with Laboratory Granulation Data 4.4.5 Summary 4.5 Granulation Behaviour for Deformable Granules: A Growth Regime Map 4.6 Control of Growth and Consolidation for Particle Design 4.6.1 Elastic Granule Systems 4.6.2 Deformable Granule Systems 4.7 Bibliography 4.8 Nomenclature
69 69 70 70 70 71 72
75 78 82 84 86 88 89 91 92 93 94 97 98 98 102 103 105 107 107 112 112 113 118 119
Breakage and Attrition 5.1 Breakage of Wet Granules 5.1.1 Experimental Observations 5.1.2 Predicting Conditions for Breakage 5.1.3 Controlling Granule Attributes through Breakage 5.2 Attrition and Fracture of Dry Granules 5.2.1 Fracture Properties of Dry Granules 5.2.2 Measurements of Fracture Properties 5.2.3 Empirical Crush Strength and Attrition Tests 5.2.4 Breakage Mechanisms for Dry Granules 5.2.5 Case Study – Fluid Bed Attrition of Agglomerates
121 121 124 125 126 126 128 131 132 134
xi 5.3 Particle Design for Controlling Attrition and Breakage 5.3.1 Effect of Process Variables 5.3.2 Effect of Formulation Properties 5.3.3 Controlling Granule Dispersibility 5.4 Concluding Comments 5.5 Bibliography 5.6 Nomenclature 6
Mathematical Modelling of Agglomeration Processes 6.1 Derivation of the Macroscopic Population Balance 6.1.1 Moments of the PB 6.2 Kinetic Expressions for Granulation Rate Processes 6.2.1 Nucleation 6.2.2 Layering 6.2.3 Coalescence 6.2.4 Consolidation 6.2.5 Attrition and Breakage 6.2.6 The Complete Population Balance for Granulation 6.3 Solution of the Population Balance Equation 6.3.1 Analytical Solutions 6.3.2 Numerical Solutions 6.4 Example Applications of the Population Balance 6.4.1 Growth by Layering 6.4.2 Growth by Coalescence 6.4.3 Effect of Mixing in the Granulator 6.5 Summary 6.6 References 6.7 Nomenclature
144 148 149 150 151 152 155 155 156 157 157 159 162 162 164 167 169 169 170
Classification and Choice of Size Enlargement Equipment 7.1 Classification of Size Enlargement Equipment 7.2 Future Directions in Granulation Process Equipment 7.3 Bibliography
135 135 137 139 140 140 141
176 177 178
Tumbling Granulation 8.1 Introduction 8.2 Disc Granulators 8.2.1 Granule Hold Up, Mixing and Segregation on the Disc 8.3 Drum Granulators 8.3.1 Granule Hold Up, Mixing and Segregation 8.3.2 Granulation Drum Circuits 8.4 Granulation Rate Processes 8.4.1 Nucleation 8.4.2 Consolidation 8.4.3 Granule Growth by Coalescence 8.4.4 Layering
179 179 180 184 185 185 186 186 187 188 191
xii 8.5 8.6 8.7 8.8 9
Scale Up and Operation of Tumbling Granulators Variations on a Theme Bibliography Nomenclature
192 194 194 194
Fluidised Granulators 9.1 Hydrodynamics of Fluidised Beds 9.1.1 Minimum Fluidisation Velocity and Pressure Drop 9.1.2 Types of Fluidisation Behaviour 9.1.3 The Role of Bubbles in Fluidised Beds 9.2 Mass and Energy Balances 9.3 Granulation Mechanisms and Rate Processes 9.3.1 Nucleation 9.3.2 Coalescence 9.3.3 Layering 9.3.4 Consolidation 9.3.5 Attrition 9.3.6 Summary 9.4 Scale Up of Fluidised Bed Granulators 9.5 Operation of Fluidised Bed Granulators 9.6 Draft Tube and Spouted Bed Coaters 9.7 Concluding Comments 9.8 Bibliography 9.9 Nomenclature
198 200 201 202 204 205 206 208 211 211 212 212 213 214 215 218 219 219
10 Mixer Granulators 10.1 Introduction 10.2 Description of Mixer Granulation Equipment 10.2.1 High Shear Mixer Granulators 10.2.2 Low Shear Mixer Granulators 10.3 Powder Flow in Mixer Granulators 10.3.1 Powder Flow in a Vertical Shaft Mixer 10.3.2 Powder Flow in Horizontal Axis Lodige Granulator 10.4 Granulation Rate Processes in Mixer Granulators 10.4.1 Wetting and Nucleation Case Study 1 10.4.2 Consolidation and Growth 10.4.3 Granule Breakage 10.5 Scale Up of Mixer Granulators 10.5.1 Scale Up of a Vertical Shaft Mixer Case Study 2 10.6 Instrumentation and Control in Mixers 10.7 Summary 10.8 Bibliography 10.9 Nomenclature Index
221 222 222 226 226 227 228 230 230 232 234 235 237 238 240 242 246 246 247 249
THE SCIENCE AND ENGINEERING OF GRANULATION INTRODUCTION Fine powders are a pain. They are difficult to handle and to process. Granulation converts fine powders to granular materials with controlled physical properties. Granulation and related processes cover a wide range of techniques used to form agglomerates that range in size from ∼100μm to 20mm and varying in structure from loose aggregates to dense compacts. Sometimes even the fine powder feeds are avoided with granules formed from liquid (solution, slurry, melt) feed. Particle size enlargement techniques are used in every processing industry which handles particulate feeds, intermediates or products. This in itself is testimony to the value of the operation. Table 1-1 summarises the many reasons for granulating fine powders. Table 1.1. Why granulate? Reason
To produce useful structural forms To provide a defined quantity for dispensing and metering To eliminate dust handling hazards or losses To improve product appearance To reduce caking and lump formation To improve flow properties for further processing To increase bulk density for storage To control dispersion and solubility To control porosity and surface-to-volume ratio To improve permeability for further processing To create non-segregating blends of powder ingredients
powder metallurgy agricultural chemical granules, pharmaceutical tablets briquetting of waste fines food products fertilisers pharmaceuticals, ceramics detergents instant food products catalyst supports ore smelting ore smelting, agricultural chemicals, pharmaceuticals
A word about linguistics. Many terms are used for the variety of industrial size enlargement processes. These include agglomeration, granulation, pelletisation and balling. Terminology is very industry specific, so let’s be clear. In this book we divide size enlargement processes into two categories (figure 1-1): • Granulation uses a liquid binder to form interparticle bonds and agitates the powderliquid mass to promote liquid dispersion and granule growth. This class of processes include fluidised beds, tumbling drums and pans, and mixer granulators. • Compression processes use pressure to promote interparticle bonds. These processes are often performed dry. Where liquid is added, it is to enhance powder flow. This class of processes include roll pressing, extrusion (dry or wet), tabletting and briquetting. 1
We will call the agglomerated product from a granulation process granules. The formulation is the combination of powder and liquid feed materials to the granulator. Table 1.2. Size-Enlargement Methods and Application Method
Tumbling granulators • Drums • Discs Mixer and Planatary granulators • Continuous high shear • Batch high shear Fluidized granulators • Fluidized beds • Spouted beds • Wurster coaters Centrifugal granulators Spray methods • Spray drying • Prilling Compression agglomeration • Extrusion • Roll press • Tablet press • Molding press • Pellet mill
Fertilisers, iron ore, non-ferrous ore, agricultural chemicals Chemicals, detergents, carbon black Pharmaceuticals, ceramics Continuous: fertilisers, inorganic salts, detergents Batch: pharmaceuticals, agricultural chemicals, nuclear wastes Pharmaceuticals, agricultural chemicals Instant foods, detergents, ceramics Urea, ammonium nitrate
Pharmaceuticals, catalysts, inorganic chemicals, organic chemicals, plastic preforms, metal parts, ceramics, clays, minerals, animal feeds
This book focuses primarily on granulation. Table 1.2 lists the key size enlargement processes and some typical applications. Chapter 7 gives more details on the range of particle size enlargement processes, their applications and idiosyncrasies. Within a process plant, the size enlargement circuit also includes a number of peripheral operations such as milling, blending, drying and classification (figure 1-2). In general, the size enlargement operation cannot be considered in isolation. Interactions with the other processes must be taken into account. Historically, granulation circuits have been designed and run based on no science, a little bit of empirical engineering and a lot of art. However, our understanding of powder mechanics is greatly improved. Sophisticated techniques to characterise formulations and granules are available both in the laboratory and in the plant. This book is devoted to developing a sound scientific and engineering approach to design, scale up and operation of size enlargement processes. The remainder of this chapter introduces the conceptual framework that we will use to achieve this.
THE SCIENCE AND ENGINEERING OF GRANULA nON
(x or y) ;;; (size, "oidage" s trength,
.surface properties, Cluulity metric)
Feed Compression vessel (x Or y)
~ (siz., ,·oid"g.. strength,
tlrrace l)fOpertlcs, qUll llty metric)
%1 / \
Figure 1.1. The unit-operations of (a) granulation and (b) compression agglomeration. X and Y represent a set ofparticle attributes, such as size and porosity. E represents additional process streams such as spray rates of moisture or slurry, steam, or heated air. P represents a description of the applied compression stress, such as maximum applied load and the rate and duration of load
Figure 1.2. A typical size enlargement circuit for pharmaceutical or agricultural chemicals involving both granulation and compression techniques
1.1. Granulation Rate Processes Granulation is a complex process with several competing physical phenomena occurring in the granulation vessel, which lead ultimately to the formation of the granules. We will divide these phenomena into three groups of rate processes (figure 1-3): 1. wetting, nucleation and binder distribution 2. consolidation and growth 3. attrition and breakage The first stage of granulation is the addition and distribution of the binder to give nuclei granules. This occurs within the liquid spray zone in the granulator. The liquid binder is usually sprayed onto the moving powder bed. Ideally, each drop will imbibe into the powder bed, engulfing particles to form a single granule nucleus. If the drop does not easily wet the powder, or the rate of imbibition is slow, large wet agglomerates will form at the powder surface. Sometimes shear forces within the powder bed are large enough to break up these clumps of wet material to further distribute the liquid. Nucleation gives a distribution of loosely packed granule nuclei. Under good wetting conditions, the distribution will be narrow and correlate closely with the liquid drop size distribution. Poor wetting and nucleation causes a broad nuclei size distribution and often poor final granule properties. The nucleation process is strongly influenced by the characteristics of the liquid spray, the flux of powder through the spray zone and the wetting properties of the formulation.
THE SCIENCE AND ENGINEERING OF GRANULATION
Granule nuclei will consolidate through collisions with other granules, and granulator. The extent of consolidation depends on the intensity of agitation in the granulator and resistance of the granule to deformation. Granules made from fine powders or with viscous liquid binders resist deformation on impact and consolidate slowly. Granules made from coarse powders deform a lot on impact and quickly reach their minimum porosity. Granule consolidation controls the final granule porosity which influences many other granule properties. When two granules collide they may stick together to form a single large granule. This is growth by coalescence. For successful coalescence (a) the energy of impact must be absorbed during collision so that the granules do not rebound; and (b) a strong bond must form at the contact between the colliding granules. The presence of liquid at the surface of the granule is important for growth by coalescence and coalescence rate is very sensitive to liquid content. Consolidation and coalescence are closely related and are considered together in this book. Granules formed through a combination of nucleation and growth processes are eventually dried. The dry granules may break to give several fragments or attrit to give a fine powder. These processes are controlled by the fracture mechanics of the granule. Granules resist attrition if their fracture toughness is high (related to formulation properties) and the number and size of flaws is small (related to granule porosity). These rate processes are at the heart of the granulation process and determine the final granule properties. It is important to know which rate processes dominate in any particular application. For example, if nucleation is the dominant rate process, adjusting the liquid spray nozzles will have a profound effect on granule size distribution. If coalescence rates are high, granule size will be very sensitive to liquid content and granule residence time. We therefore spend a lot of time examining each of these processes in detail. We will: examine the underlying physics behind each rate process • • define the controlling formulation properties and process parameters for each rate process • use regime maps to establish the operating regime for the granulator provide quantitative relationships to predict the effect of changing operating • parameters and formulation properties provide troubleshooting and scale up guidelines •
Figure 1.3. Rate Processes in Granulation (a) wetting and nucleation; (b) consolidation and growth; (c) breakage and attrition
1.2. Considering a Granulator as a Reactor There is an analogy between a granulation process and a chemical reactor. A chemical reactor converts feed materials to different chemical species via a series of chemical reactions. A granulator converts fine powders to granules via a series of physical rate processes. Chemical reactor engineering is very well established. We can apply many of the methologies from reaction engineering to approach granulator design. There are four natural scales of analysis for a granulator or reactor (figure 1-4): 1. Particle scale: A granule is an agglomerate of many small particles. The granulation process depends ultimately on the particle-particle and particle-binder physicochemical interactions at a small scale. This is analogous to examining chemical reactions at the molecular level. 2. Volume of powder scale: Within some volume element in the granulator, we define the physical rate processes that are occurring (nucleation, coalescence, etc.). Kinetic expressions are written for rate process which give the rate of change of granule properties eg. size distribution. This is analogous to writing rate expressions for several chemical reactions in a reactor. 3. Granulator scale: A series of balance equations is written to describe the evolution of the granule property distributions in the granulator. These equations incorporate rate
THE SCIENCE AND ENGINEERING OF GRANULATION
expressions for each of the physical rate processes, residence time distributions and mixing patterns in the granulator. The mass, energy and population balances for a granulator are equivalent to the total mass, energy and individual component balances for a reactor. 4. Granulation circuit scale: The performance of a chemical reactor cannot be considered in isolation. Products need to be separated after reaction. Unreacted feed needs to be recycled. In the same way, design and operation of granulation circuits requires consideration of all the unit operations and their interactions. Note that most granulation plants are either batch operations or continuous operations with large recycle. Both cases provide special problems for process control. Good engineering requires investigation at all four scales. Furthermore, knowledge and models at all scales of analysis should be linked. Rate expressions for physical rate processes (volume of powder scale) are of limited value unless they are sensibly derived from underlying phenomena at the particle scale. Granulator performance may be dominated by the properties of recycle materials to the reactor. While this may seem commonsense, it is rarely applied in practice. In this book we will use the reactor analogy and reaction engineering methodology extensively. A lot of emphasis is placed on linking the four scales of analysis.
Figure 1.4. Comparisons of scales of analysis of chemical reaction and size-enlargement processes
1.3. Granulation as Particle Design Granulation should be used to produce granules with defined properties to meet specific end use requirements. Key primary properties are granule size distribution and porosity. These two properties which dominate a wide range of secondary properties may also be important, depending on the application. Achieving the desired designer particle is a combination of process engineering and product engineering. Process engineers choose processes and manipulate process variables to change the granule properties. Product engineers manipulate the ingredients or formulation to achieve the same effect. Let's illustrate the particle design concept with an example. Herbicide and pesticide powders must be dispersed in water by the farmer before spraying onto crops. Small particle size is needed so the particles don’t settle out in the tank (of order a few microns). However, fine powders are hard to disperse in the water. They are dusty, cake in the bag and can be inhaled by the farmer. The designer particle must therefore have the following properties: • • • •
easy to handle non-dusty strong enough to avoid attrition during handling disperses in water to a stable colloidal suspension within seconds
Several companies now produce these designer particles commonly known as water dispersible granules (WDGs). The granules are made from finely milled powder (for final suspension properties). The fine powder is granulated with water to produce porous free flowing granules. The large granules will break the surface of water in the tank easily and disperse to their unit particles as water enters the granule. To achieve the desired properties, clays and surfactants are added to the formulation to help granules disperse once they are wet. Additional binders may be added to give the granules dry strength during transportation. Several different granulation techniques have been used to produce WDGs. It is critical in processing to control the granule porosity. If the porosity is too low, the granules will not disperse in water; too high, and granules attrit to produce dust during handling. Other process issues affect the granule properties eg. if the residence time during drying is too long, the surfactant will age leading to poor dispersion. Control of both process variables and formulation properties is necessary to achieve the desired WDG properties. In any granulation process, process variables and formulation properties interact to give the final particle design. Often, different groups in a company are responsible for formulation design and process design/scale up. If these two groups do not interact, problems are likely to occur! This lack of interaction has also occurred in the scientific literature on granulation.
THE SCIENCE AND ENGINEERING OF GRANULATION
Good particle design requires four things: 1. 2. 3. 4.
Clear definition of the required granule properties. Good characterisation of formulation ingredients and granules. Understanding the impact of formulation properties on granule properties. Understanding the impact of process choice and operating variables on granule properties.
In this book, granulation is approached from a particle design perspective. There is a heavy emphasis on (a) defining and measuring both formulation and granule properties, and (b) how granule properties are evolved from the interaction between formulation properties and process variables.
1.4. How To Use This Book The aim of this book is to provide a scientific and engineering basis for design and operation of granulation processes. It is divided into two parts: • Part A: Granulation Process Fundamentals • Part B: Equipment Selection, Design and Operation In Part A we examine the underlying phenomena that control the granulation process at the particle and volume of powder scale of investigation. Chapter 2 defines important properties of particles and particle assemblies. Chapters 3 to 5 examine each class of rate process for granulation.. Each chapter describes the physics that control the rate process and relevant characterisation techniques for formulation and granule properties. Rate expressions are developed in terms of equipment independent process parameters. Examples from different types of equipment are used to illustrate the concepts and a summary table presented on ways to control the rate process. Part A finishes with the mathematical description of rate processes to predict the evolution of granule property distributions in the granulator (Chapter 6). Part B analyses granulation at the granulator and granulation circuit scale. Chapter 7 classifies and compares different granulation and compression agglomeration techniques. This chapter gives a rationale for equipment selection. The following chapters each focus on an individual technique, giving brief descriptions of equipment and looking at equipment specific design, scale up and operation. These chapters refer heavily to the understanding developed in Part A to describe and quantify the rate processes for the technique being studied. Readers can begin with either Part A or Part B. Researchers and formulation designers may wish to start at Chapter 2 and gradually build up a fundamental understanding of the rate processes and underlying science. Process engineers and technologists in manufacturing who want to get a broad overview or focus on one type of equipment only, may start with Chapter 7 and refer back to Part A only as indicated in the equipment specific chapters.
CHAPTER 2 PARTICLE AND GRANULE MORPHOLOGY “Measure Properties, don’t perform rituals’1 Good particle design means understanding particle-particle and particle-fluid interactions and using this knowledge to properly design processes and products. It is the properties of the particle that dictate these interactions so particle characterisation is at the heart of particle design. Good characterisation of both the feed powders and the product granules is essential. However, particle characterisation presents special challenges that don’t exist for the measurement of fluid properties: • •
The discrete nature of a particulate system means that it is heterogeneous. Two particles in the same system don’t have the same properties. We need to measure property distributions and sampling is a major issue. The properties of particulate systems can’t be tabulated like the thermodynamic properties of fluids. The properties of the system depend not only on the chemical composition, but also the particle morphology. You can’t look up surface area of sand in The Handbook of Chemistry and Physics! You have to measure it. The properties are not always easy to define. The simplest example of this is particle size (see below). Historically, many particle properties have been difficult and time consuming to measure.
These challenges have led many practising engineers and technologists to “perform rituals” rather than measure properties. These rituals measure some empirical parameter that may bear no relationship to any fundamental property, but involve tests that can be easily and routinely performed. Such rituals are enshrined in company and industry standards. The need for these rituals is gone. Effective on-line and off-line measurement of real properties is now possible with modern particle characterisation techniques. Figure 2.1 illustrates some important particle properties. The particle properties determine the macroscopic properties of the particle assembly or bulk solid. We cannot yet predict completely bulk solid properties from knowledge of particle properties so that ability to define and measure bulk solids properties is also important. Each chapter in the first part of this book defines important particle or granule properties and discusses their measurement. This chapter focuses on the morphological properties - size, shape, density and porosity. All other granule attributes are a strong function of these properties so they need to be defined clearly at the start. We first define the properties for any particle. At the end of the chapter we look at special issues associated with granule morphology.
From a speech by Roland Clift to the 1st International Particle Technology Forum, Denver 1994.
Particle characterisation is a book in itself and that book has already been written (Allen, 1997). You should refer to Terry Allen's excellent book for a more detailed discussion of the topic.
Surface active agents Surface Energy
E Electric.al &
Toughness Hardness Elastic Moduli
Figure 2.1. Particle properties affecting particle and assembly behavior
2.1. Particle Size, Shape and Size Distribution 2.1.1. Particle Size Definitions Size is the single most important property of a particle in a formulation. It defines the basic building block of the granule. Particle size strongly influences other important particle and granule properties (Table 2.1). One reason for this is that size controls the balance between surface forces and body forces with the surface forces becoming increasingly dominant as size becomes small. So knowledge of the particle size of a system is essential. However, real life is not that simple. There is no clear definition of particle size for real (irregularly shaped) particles. In practice, there are many definitions of particle size. Some of the most important are "equivalent diameters". The equivalent diameter is the diameter of a sphere with the same property as the particle ego the volume equivalent diameter is the diameter of a sphere with the same volume as the particle:
PARTICLE AND GRANULE MORPHOLOGY Vp =
Similarly, the specific surface area equivalent diameter is defined by:
( S / V ) p = 6 / d sv
Often, size is not measured directly. Instead, a size dependent property is measured and the size is inferred. For example, settling velocity may be measured and the size calculated from Stokes Law. In this case the measure of size is the Stokes diameter dSt , ie. the diameter of a sphere with the same settling velocity as the particle. Table 2.2 gives ten examples of different measures of particle size. Ideally, the choice of particle size measurement should match the application. There is no clear choice for granulation formulations and volume equivalent diameter and sieve diameter are the most commonly used. The specific surface diameter (eqn. 2-2) is also an important measure, especially for fluidised bed granulators and driers. 2.1.2. Particle Shape Particle shape affects flowability, packing density and particle-fluid interactions. Shape is more difficult to define and measure than particle size. Qualitative descriptions are available but are not useful for quantitative calculations. One useful quantitative measure of shape is the shape factor. The shape factor relates some property of the particle to a measure of particle size. For example, the volume shape factor, surface ar ea shape factor and specific surface shape factor is defined by the equation: V p = α v x 3 ;S p = α s x 2 ;(S / V ) p =
α sv x
Table 2.1. Properties of particles, granules and particle assemblies that depend on particle size Property
Properties of single particles 1. Homogeneity 2. Elastic-plastic behavior (ductility) Probability of breakage Particle strength Wear behavior
Trend with decreasing size
Other relevant particle properties
Decreasing Increasing Decreasing
Toughness Hardness Flaw distribution
Surface energy Charge distribution Surface groups Impurities Hardness Surface asperities Density Shape Interparticle forces
1. Bulk density
2. Rheological behavior: elasticity, yield point,
3. Wetting 4. Strength of agglomerates & briquettes 5. Powder mechanics: shear stress, unconfined yield stress, cohesive stress, wall friction 6. Fluid-mechanics: permeability, fluidizability 7. Ignitability, explosive behavior
Density, shape, friction, interparticle forces Size distribution, density, shape, interparticle forces, friction Surface energy, contact angle Fracture toughness, hardness, elasticity voidage, flaws Surface energy, friction, asperities, hardness, elasticity
8. Reactivity, solubility (e.g. taste, activity)
3. Properties resulting from competition between volume and surface forces, e.g.: adhesion agglomeration suspendability
Properties of particle assemblies and granules
Usually decreasing Increasing
Density, interparticle forces Chemical and surface properties Surface energy Flaw distribution
PARTICLE AND GRANULE MORPHOLOGY
Table 2.2. Nine typical measures ofsize or length scale for irregularly shaped particles
Particle under study
Direction of measurement
Diameter of a sphere having the same volume as the particle Vp
Diameter of a sphere having the same surface area as the particle S p =
Stokes' (or drag) diameters
Diameter of a sphere having the same terminal velocity as the particle
g(pp - p)dl,
Specific surface diameter
Diameter of a sphere having the same specific surface area as the particle (S / V) p =6 / d sv
Particl sieve diameter
Width of the minimum square aperture through which the particle wi ll pass
Projected area diameter
Diameter of a sphere having the same projected area as the particle Ap
Projection of the particle's outline onto a line perpendicular to the direction of measurement
Chord parallel to the di rection of measurement wh ich bisects the projected area
Diameter of a sphere scattering Ii ht at the same intensi
Note that the numerical value of the shape factor depends not only on the particle shape but also on the definition of particle size x. One shape factor deserves special mention. It is the particle sphericity lfI which is defined as: surfaceareaof aspherewithsamevolume suifaceareaof the particle
As a sphere is the shape with minimum surface area, the maximum value of lfI is 1. Low values of lfI indicate large deviations of particle shape from spheres ego needles, fibres and plates. More complex defmitions for particle shape include the fractal dimension of the particle. This is particularly useful for floes and loose particle aggregates. We can estimate the relationships between different particle size definitions if the particle shape is known. From the definition in eqn. 2-4: dv
= rIIEO . 5 d s
A very useful approximate relationship between sieve size and equivalent volume size is : (2-6) Particle shape is measured directly by microscopy combined with image analysis, indirectly by measuring particle size by two different techniques or by light scattering techniques.
PARTICLE AND GRANULE MORPHOLOGY
2.1.3. Basic Particle Size Distribution Definitions
Particle size (and other properties) present a further problem. They do not have single values. Instead there is a distribution of values of the property and we need to be able to define and describe these distributions. There are two ways to represent the particle size distribution : • a cumulative distribution: The cumulative distribution, N(x), is the number of particles less than size x. • a frequency distribution: The frequency distribution, n(x), is defined such that n(x)dx is the number of particles between sizes x and x+dx Clearly, N(x) and n(x) are related. From their definitions: N ( x) =
³ n( x ′)dx ′; 0
n( x ) =
d N ( x) dx
Figure 2.2 shows the relationship between the frequency and the cumulative size distributions. From the definition of the frequency size distribution, it follows that the total area under the n( x ) curve must be N T , the total number of particles: ∞
³ n( x)dx = N 0
We often express the cumulative and frequency distributions as normalised distributions (see figure 2.2): f ( x) =
n( x ) ; NT
F ( x) =
N ( x) NT
Note that the frequency distribution f (x) has the dimensions L-1 e.g. units of m-1. The fraction of particles in a size range is represented by the area under the curve of the distribution. We can't define the number of particles of size x, only the number between two sizes, x and x+dx. When viewing size distribution data, always plot the true frequency distribution, not the fraction in a size interval against size. Equations 2-7 to 2-9 are written for a continuous distribution. In practice, we usually measure size distributions divided into sections or intervals. Each size interval is defined by the largest size in the interval ( x i ) and the width of the interval ( Δxi = xi − xi −1 ). Within each interval, we assume constant values for particle properties e.g. the particle frequency (see figure 2.3). We can rewrite all the size distribution definitions for a sectional distribution. Table 2.3 summarises the relationships between the standard ways of representing particle size distributions.
Figure 2.2. Cumulative and frequency size distributions
PARTICLE AND GRANULE MORPHOLOGY
Table 2.3. Summary of size distribution definitions
Type of distribution
N ( x) n( x )dx
no. of particles less than size x no. of particles between size x and x + dx
F ( x)
f ( x )dx
no. fraction of particles less than size x no. fraction of particles between size x and
³ n( x)dx = N 0
maximum size of particles in size interval
n *i = n i Δ x i
³ f ( x ′)dx ′ 0
d f ( x) = F ( x) dx ∞
³ f ( x)dx = 1 0
d n( x ) = N ( x) ; dx
n( x ) N ( x) ; F ( x) = NT NT
f ( x) =
Δxi = xi − xi −1
³ n( x ′)dx ′
F ( x) =
x + dx
N ( x) =
width of size interval
N i = ¦ n*j = ¦ n j Δx j ni Δxi =
no. of particles in size interval i
= N i − N i −1
¦ n Δx i
no. of particles in all intervals up to and including i
n( x )dx Δxi
; N i = N ( xi )
CHAPTER 2 Normalised/sectional no. fraction of particles in all intervals up to and including i
Fj Yi =f/1xi
i = LYj = LfjL1xj j=! j=!
f/1xi = Yi = Fj -
no. fraction of particles in size interval i
LfiLlxi =1 i=l
[' f(x)dx fi =
;Fj = F(xJ
size interval i area = number fraction in size interval Frequency size dist.
Particle Size Figure 2.3. Frequency histogramfor a discrete size distribution
2.1.4. Different Ways to Represent Particle Size Distributions
So far, we have looked at the distribution of number of particles with size x. However, we may generalise the analysis and represent a distribution of any measure of quantity of particles with any property. We write a generalised distribution as fa (.;) where ~ is the particle property of interest and the subscript a denotes the measure of quantity of particles. fa (.;) is defined such that the fraction of the amount of a between ~ and
PARTICLE AND GRANULE MORPHOLOGY
~+ d~ is fa(qyd~. When plotting the distributions, the quantity is the y-axis variable and
the property is the x-axis variable (see figure 2.4). When the quantity a is the number of particles we usually omit the subscript. The most common alternative quantity used is mass (volume) because many sizing techniques measure the mass of particles, rather than count the number.
Partice size, x
(or other property)
Figure 2.4. Examples of different frequency size distributions
Apart from the linear size x, other choices for the property ~ are particle volume and log of particle size. The logarithmic frequency distribution is very useful where data is collected for geometric size intervals ie. Xi = kx i - l . Common values of k are 2, .J2 and
ifi. In principle, we can readily convert from one type of distribution to another. Table 2.4 gives common conversions to change either the property or the quantity of the distribution. These relationships can be derived directly from the size distribution definitions (see Allen, 1997). Despite the fact that converting distributions from one form to another is mathematically straightforward, great caution should be shown in manipulating the measure of quantity for real data. The reason is clear from figure 2.4. Volume distributions give much greater weighting to the large particle end of the distribution where there are very small numbers of particles and the error in the number size distribution is very large. The errors in converting real broad size distribution data from a volume (mass) basis to number basis can be extremely large. A quick look at Tables 2.3 and 2.4 show an impressive list of different symbols and definitions. In fact, most of the difficulties in handling size distributions come from confusion in definitions and nomenclature.
Table 2.4. Converting between different distributions
f ( x)
x f ( x) 2
f s ( x) =
f si =
x f ( x ) dx
xi 2 f i
f j Δx j
f ( x) =
f s ( x)
x i f si
f sj Δx j
f ( x ) dx
x 3 f ( x)
f v ( x) =
volume or mass
f ( x)dx
f vi =
f ( x) =
x i fi
f v ( x)dx
f j Δx j
x − 3 f v ( x) ∞
f vj Δx j
f ( x)
f (v ) =
f (ln x) = xf ( x)
3α v x
fi 3α v x i 2
f i ln x = xi f i
2.1.5. Measures of Mean Size and Spread of the Size Distribution A full size distribution is a lot of information to carry around and manipulate. It is useful to define a limited set of parameters that characterise the whole distribution. We start by defining the un-normalised moments of the number-size distribution: ∞
μ k′ = x k n( x)dx =
¦x i =1
k i ni Δx i
PARTICLE AND GRANULE MORPHOLOGY
The total number and volume of particles are related to the zeroth and third moment: N T = μ 0′ VT = α v μ 3′
A general definition of “mean size” is also written in terms of the moments:
§ μ′ = ¨¨ m © μ n′
· m−n ¸ ¸ ¹
There is no unique mean size that reveals everything about the distribution. Important examples of mean sizes based on this definition are: •
x1,0 = μ1′ / μ 0′
x3, 2 = μ 3′ μ 2′ (the specific surface or Sauter mean)
x 4,3 = μ 4′ μ 3′ (the mass-moment or volume-moment mean)
The key point is to use the mean size relevant to your application. For example, the specific surface mean x32 should be used to calculate the surface area per unit volume of the powder:
(S / V ) =
α sv x 32
Any other mean size used in eqn. 2-14 will give the wrong answer. Different measures of mean size will vary widely for a broad size distribution. An alternative approach is to define measures of average size and spread of the size distribution in terms of values related to the cumulative distribution: • •
the median size x50 is the 50% passing size ie. F ( x50 ) = 0.5 . the range of the distribution is the difference between the 95% passing size and the 5% passing size ( x 95 − x 05 ).
2.1.6. Particle Size Measurement
A wide range of techniques are used for particle size analysis. The choice of technique depends on the application. Some techniques measure particle size directly, while others measure a property that depends on particle size. Table 2.5 shows a number of commonly used particle sizing methods (see Allen for more exhaustive descriptions). For particles above 0.1 mm in size, sieving is easily the most popular technique. For finer sizes there is
no single best methods although light diffraction techniques are common because of the speed and ease of the measurement. Measuring particle size distribution correctly takes some skill. There are some important points to remember: 1.
Getting a representative sample is vital. Without a representative sample, correct sizing is impossible. Often, much more effort is required in getting the sample than in doing the size analysis. Use extreme caution when comparing size distributions measured by different techniques as they may be measuring different particle sizes. If possible use a technique that measures the “size” you want to know e.g. microscopy is a good technique for sizing paint pigment because projected area is the property of interest. If fine dust is present in the sample, dry sizing techniques will give a different size distribution to wet sizing techniques because the dust adheres to the larger particles. In particular, beware of dust blinding screens for dry sieve analysis. It may be necessary to “deslime” the sample over a fine screen first. If you need the number size distribution use a technique that counts particles. If you want the mass size distribution use a technique that measures mass directly. Very large errors can occur from converting from one form of the size distribution to the other.
Never accept size analysis data on face value. Always view the data critically in light of the comments made above.
2.1.7. Particle Size Summary
Particle size is the single most important property of a particulate system, hence the detail it has received in this chapter. Size is also a good case study for common issues and problems associated with any particle property. In summary: • • • •
There is no single definition of particle size. Know the common definitions and be sure you know what “size” you are talking about. Size distributions can be represented as cumulative or frequency distributions. Be comfortable with the mathematics of size distributions and common transformations eg. converting from mass to number size distributions. There are many definitions of mean size. Choose the definition appropriate to your application. There are many ways to measure size and size distributions. They measure different types of particle “size” and different types of size distribution. Correct sampling and sample preparation are very important. Never take particle sizing data at face value. View it with a critical eye.
PARTICLE AND GRANULE MORPHOLOGY
Table 2.5. Commonly employed methods of particle size analysis
Microscopy Optical Electron (e.g.TEM,SEM) Image analysis Sieving Wire woven Electro-formed Sedimentation Micromerograph Pipette extraction Photosedimentation X-ray sedimentation Sediment balance Elutriation/cyclone tech. Sensing zones Electrical (e.g Coulter) Optical: Scattering Diffraction (e.g. Sympatec Helos or Malvern) Obscuration Surface methods Surface permeametry Gas adsorption Thermal conductivity Adsorption from solution Heats of solution/wetting Miscellaneous Ultrasonic attenuation Photon correlation spect. Scanning IR laser (e.g. Lasentec Labtec 100)
Size range [m]
Particle size measured
Type of distribution
Cost range [$] On-line capability(+)
Dry or wet Dry Dry or wet
A range of geometric diameters
100-2000 30,000-250,000 3,000-150,000 (+)
Dry or wet Dry or wet
5-75 2-75 2-75 (.05-5 centrifugal) .1-75 (.05-5 centrifugal) 2-75 2-100
Dry/gravity Wet/gravity or centrifugal " " " " Dry or wet
Mass Mass Surface Mass Mass Mass
15,000 60 1000-5000 (25,000 centr.) 10,000-20,000 3000-8000 (+)
Wet Wet or dry
Scattering diam. Scattering diam.
Number or vol. Volume
20,000-50,000(+) 50,000-90,000 (+)
Proj. area diam.
Dry Dry Dry Wet Wet
1-500 .003-3 m
Volume diameter Scattering diam.
30,000-50,000 (+) (+)
2.2. Density, Porosity and Pore Size Distribution 2.2.1. Density and Porosity Definitions
Powder density is an important property in determining requirements for granulation. In fact, granulation may be primarily for the purposes of either increasing or decreasing powder density. For any particle assembly, there are three important densities to define for a given mass of solid M (see figure 2.5). The difference is in the reference volume used. The three densities are: • bulk density: which relates to the volume occupied by a bulk solid including all void space. • particle (apparent) density: which relates to the volume occupied by a single particle including internal porosity. The volume is defined by an imaginary envelope around the particle. • skeletal (true) density: this is the true solid density of the material.
Figure 2.5. Different types of solid density
Only the third of these is a property of the material that can be tabulated. Bulk density and particle density are strong functions of particle morphology (size, shape, porosity). Bulk density is an important property in determining bulk solid storage and handling requirements. Particle density is important in determining the interactions between particles and fluids. The three densities are related by the fraction of the volume occupied by the fluid. We define the voidage ε as the fraction of bulk solid volume present as voids between particles. The porosity ε pore is the fraction of particle volume present as pores within the particle. Table 2.6 summarises all the density and porosity definitions. The densities, voidage and porosity are related as follows: ȡ p = ȡ b (1 − İ )
ȡ s = ȡ p 1 − İ pore
PARTICLE AND GRANULE MORPHOLOGY
Table 2.6. Density, porosity and voidage definitions Property
M V s + Vv + V p
particle (apparent) density
M Vs + V p
skeletal (true) density
Vv V s + Vv + V p
Vp Vs + V p
M = solid mass; Vs = solid volume; Vv = void volume in particles; Vp = pore volume
2.2.2. Density measurement
The general principle in density measurement is to measure the volume occupied (or fluid volume displaced) by a known mass of solid. Solids preparation is critical. The measured density is a strong function of the way the sample is prepared. Bulk density is relatively easy to measure by simply observing the volume taken up by a known mass of bulk solid. The loose filled bulk density is measured immediately after pouring into the container. This is not a very reliable measurement. The tapped bulk density measures the volume occupied by the bulk solid after tapping the container mechanically till it reaches it maximum settled density. For fine solids, bulk density may increase significantly under pressure. The compressibility of fine solids will be considered further in the section on bulk solids characterisation. Skeletal (true) density is measured by the volume of a liquid or gas displaced by the solid. The density is measured with a liquid or gas pycnometer. Standard techniques are available and well documented eg. BS 3483, Part B8 (1978). In both cases, sample preparation is critical. For a liquid pycnometer it is important the liquid chosen completely wets the solid. The solid is first ground finely and evacuated before adding liquid. These preparation steps are aimed at ensuring that all gas in the sample is completely displaced by the liquid. In gas pycnometry, an inert gas (Argon or Helium) is used. After evacuating the sample, the volume of gas taken up by the sample at several different pressures is measured. The solid volume can be inferred from these measurements.
Particle density is the most difficult density to measure accurately. The problem is that only an imaginary envelope separates the internal pores from the external voids and the displacement fluid is not smart enough to know the difference! Techniques generally involve three steps:
1. 2. 3.
Fill all particle pores with a liquid eg. soaking in boiling water. Drain particles and surface dry. Measure volume of water displaced by the wet particles.
It is difficult to separate the fluid in the pores from the surface fluid. Thus, the techniques are very inaccurate for particles less than 1mm. For these particles, the particle density must be inferred from measurements eg. combining measurement of particle porosity and skeletal density in eqn. 2-15. 2.2.3. Porosity and Pore Size Distribution Measurement
Total porosity can be calculated from independent measurements of skeletal and particle densities (eqn. 2-15). Porosity and pore size distribution are measured directly by mercury porisimetry. This technique relies on the fact that pressure must be exerted to force mercury into the pores of a particle because the contact angle between mercury and all practical solids is greater than 90º. A known mass of powder is first evacuated then exposed to a pool of mercury. As the pressure is increased, the mercury is forced into pores of smaller and smaller size. Assuming cylindrical pores, the pore size is related to the applied pressure by the Laplace-Young equation: P=
4γ lv cos θ d pore
The volume of mercury that penetrates into the powder is measured for each pressure increment. Thus the method measures directly cumulative volume basis pore size distribution V(dpore) ie. the cumulative volume of pores per unit mass of solid greater than a size dpore. The total pore volume is V(dmin) where dmin is the size of a pore penetrated at the maximum applied pressure. The pore volume is related to porosity as defined above by:
ε p = V (d min ) ρ p ; or ε p =
V (d min ) ρ s 1 + V (d min ) ρ s
The cumulative pore size distribution can be converted to a frequency distribution if desired. The same rules for manipulation and correct representation of distributions developed for particle size distributions above also apply for pore size distributions. Figure 2.6 shows an example of mercury porosimetry data for a series of granules of the same feed formulation granulated under different conditions.
PARTICLE AND GRANULE MORPHOLOGY
Figure 2.6. Typical Mercury Porosimetry Data
Some of the limitations of the mercury porosimetry technique are: 1.
2. 3. 4.
The minimum pore size is limited by the maximum pressure applied. Typically, this is of order a few nanometers. Mercury porosimetry is not applicable for characterising microporous materials. The pores are not cylindrical and are connected. This causes hysteresis in porosimetry results. For fine powders or coarse powders with large macropores, it may be difficult to distinguish between mercury intruding into interparticle voids and intraparticle pores. Powders have heterogenous surfaces so there may be a distribution of surface energies (and contact angles) as well as of pore size.
2.3. Granule Properties
The key properties of any granule are its size and porosity. Virtually all other granule properties of importance depend directly on one or the other. Figure 2.7 shows the strong relationship between granule strength and porosity. Other important morphology dependent properties include bulk density, flowability, reactivity, permeability, dispersibility and dissolution. Granules are a particular type of particle and the techniques and definitions listed above are all applicable to granules. However, sometimes there are special issues associated with analysing granules and some of these are described below.
Figure 2.7. Relationship between granule porosity and fracture toughness for herbicide granules
2.3.1. Granule Size Distribution
The desired size range for granules is always in the sizing range for sieve analysis. Wet granules, however, present special problems for sieving: • • •
they are sensitive to handling and may either granulate further or break up before their size distribution is measured wet granules may cake on the screens or blind the screen cloth it is sometimes difficult to define what is a granule and what is a set of loosely connected particles.
Sample preparation and handling is more important for granules than for "standard" particles. One useful approach in the laboratory is to freeze the wet granules with liquid nitrogen [Hinkley et al., 1994]. The liquid nitrogen can be poured directly into the granulator to freeze the granules in situ or a sample of granules is poured into a stirred container of liquid nitrogen. The frozen granules are immediately sieved for one or two minutes in a precooled set of sieves. Granules greater than 0.25 mm can be easily sieved by this technique but smaller granules are problematic.
PARTICLE AND GRANULE MORPHOLOGY
The main preparation alternative is to dry the granules before sieving but granules may cake together during tray drying or attrit and break during fluid bed drying. Care should be taken to check if dry granules break or attrit during the sieving operation. The greatest problems occur when the final granule size distribution overlaps initial particle size distribution, the material is only partially granulated with a very broad size distribution. In all cases, the sample preparation technique used needs to be well documented and repeatable. 2.3.2. Porosity and Granule Density
The porosity of dry granules can be measured by mercury porisimetry as described above (eg. Sastry et al., 1977). Porous, friable granules may deform or crush under the pressure exerted by the mercury. Thus, a minimum dry granule strength is needed for mercury porosimetry to be applicable. As an alternative, the apparent density of wet granules has been measured successfully by displacing a non-wetting fluid with a sample of granules (Capes and Danckwerts, 1965, Hinkley et al., 1994, Iveson, 1997). The granule porosity can then be calculated as:
ε pore = 1 −
ρ gran ρ s (1 + w)
Kerosene is the non-wetting fluid of choice. Performed with care, this technique gives errors in porosity of ±2% relative error. However, the technique is only applicable to well formed granules and does not work well for very porous granules or loose aggregates Iveson, 1997. X-ray microtomography is a new technique which has great potential to give information on the internal structure of granules (Golchert et al., 2002). This approach uses technology borrowed from medical imaging with bench top equipment now available for paticle analysis. Figure 2.8 gives an example of tomography analysis of a singe granule. Note that the pore structure is very non-uniform with large macropores or flaws in some places. This technique gives potential to study in detail how the structure of granules change with processing and variations in formulation.
Figure 2.8. X-ray tomography image of a slice through a 2mm diameter granule made from 50m glass ballotini with salt solution as binder
32 2.3.3. Wet Granule Morphology
During the wet granulation process, the granule is a three phase system consisting of particles, liquid binder and air. The granulation process is very sensitive to the liquid content, more particularly to the level of liquid saturation in the granule which depends both on the amount of liquid present and the granule porosity. We define the liquid saturation as: s=
wρ s 1 − ε pore
As the granule saturation increases, the structure of the liquid phase inside the granule changes (Newitt and Conway-Jones, 1959) (see figure 2.8). At low saturations, the liquid exists as discrete pendular bridges. As saturation increases some regions of the granule will have liquid filling capillary networks. At saturation a little below 100%, the granule will be in the capillary state ie. entirely saturated in the centre of the granule but surface dry with the liquid sucked into the entrances of the surface capillaries. For s > 100%, the granule have a liquid layer on the outside. At higher liquid contents, the granules will collapse into a slurry. Granule saturation cannot be measured directly. Instead, it must be inferred from independent measurements of granule porosity and moisture content.
Figure 2.9. The structure of granules with different liquid saturations
2.3.4. Granule Performance Properties
Depending on the desired application, there are many possible performance properties that may be measured. It is in this sphere that rituals abound. Rituals may have a place in quality control but have no place in granule design and troubleshooting. For these purposes, we need to measure properties. "Attrition resistance" is a good example to illustrate the point. Empirical techniques abound by which the size distribution of granules are measured before and after simulated
PARTICLE AND GRANULE MORPHOLOGY
materials handling eg. in a pneumatic conveying circuit, in a fluid bed, in a tumbling drum. The amount of fines generated is an index of attrition. Such tests are rituals because: 1. 2. 3.
They give no information on why the batch had good or poor resistance to attrition. Results are only useful for handling conditions very similar to the test conditions and cannot predict behaviour in other handling environments. Results from different attrition index tests correlate poorly.
An alternative approach is to measure the granule properties that control its resistance to attrition eg. fracture toughness, porosity and pore size distribution. Changes to either the formulation or the process can then be targeted to overcome the problem eg. increasing residence time or process intensity will reduce granule porosity. Table 2.7 lists a number of granule performance areas and associated important particle or assembly properties. Many of these properties are discussed in detail in the ensuing chapters.
Table 2.7. Relevant properties for granule quality Performance Area
Strength, attrition resistance Bulk Solids Flow
Packaging and Storage Segregation Caking
Dispersion and dissolution
Resistance to fluid flow Appearance
Fracture toughness Hardness Porosity Internal angle of friction Wall angle of friction Unconfined yield stress Bulk density Size distribution Size distribution Moisture content Hydroscopic tendency Phase transitions
Uniaxial compression Indentation, Notched bar Mercury Porosimetry Shear cell
Contact angle Porosity, pore size distribution Dissolution rate Permeability Size distribution Shape Colour
Drying Differential Scanning Calorimetry Dilatometry Sessile drop, Washburn, Flotation, IGC
Permeameter Image analysis
A scientific understanding of granulation requires good characterisation of both feed formulation and product granules. This should be achieved by measuring particle properties rather than empirical indicies (rituals). Particle granule size and size distribution are always key properties. Take care with the definitions and measurement of particle size, correct presentation of the size distributions, and careful choice of distribution parameters. For granule sizing, special care is needed in sample preparation through drying or freezing the granules. Next to size, granule density and porosity are the most important properties. These can be measured, with care, using a combination of fluid displacement and porosimetry techniques described in this chapter. The fractional saturation of wet granules can also be inferred from these measurements. Powder and granule morphological properties are important in all aspects of granulation and compression processes. Further important properties are defined in the ensuing chapters. A final cautionary note on sampling - the most careful property measurement is useless unless it is carried out on a representative sample. Correct sampling and sample preparation are sometimes difficult, but always essential. See Allen (1997) or Gy (1979) for detailed discussion of sampling techniques.
Allen, T., Particle size measurement, 5th edition, Chapman and Hall, 1997.BS3483, Part B8 (1978). Capes, C. E. and Danckwerts, P.V.,Trans. I. Chem. Eng., 43 (1965) 116-124. Golchert, D., 2002. Proc. 6th World Congress on Particle Technology WCPT4, Sydney, July 24-28. Gy, P., Sampling of particulate materials: Theory and Practice. Elsivier Scientific Pub. Co. 1979. Hinkly, J., Waters, A.G., O’Dea, D. and Litster, J.D., Int. J. Mineral Proc., 41 (1994) 5369. Iveson, S.M., Fundamentals of granule consolidation and deformation, PhD Thesis, University of Queensland. 1997. Newitt and Conway-Jones, Transactions of the Institution of Chemical Engineers 36 (1958) 422-442. Sastry, K.V.S. and Fuerstenau, D.W., Kinetic and process analysis of the agglomeration of particulate materials by green pelletization, in: Sastry (Ed.), Agglomeration’77, AIME, New York, 1997, 381
PARTICLE AND GRANULE MORPHOLOGY
2.6. Nomenclature a c dv, ds, dsv fc f(x) fα(ξ) F(x) M Ms n(x) n*i N(x) NT P p Q r s S SE t t0.025 v V x xi
xm ,n K yi
αv, αs, αsv
γ lv , γ ls , γ sv
δ ε ρ ρb, ρp, ρs σ2 σ
arbitrary property of particles cohesion of bulk solid (Nm-2) equivalent diameters - volume, surface area, specific surface area respectively (m). unconfined yield stress (Nm-2) normalised frequency size distribution (m-1) normalised frequency distribution of property ξ with respect to quantity α normalised cumulative size distribution total mass sample mass un-normalised frequency distribution (no. m-1) number of particles in size interval i un-normalised cumulative size distribution total number of particles pressure (Pa) probability number of sample increments pore radius particle surface area (m2) surface area (m2) sampling error time t statistic particle volume (m3) volume (m3) particle size (m) maximum size of particle in interval i (m) mean size of interval i (m) width of size interval i (m) the “m,n” mean size permeability fraction of particles in size interval i shape factors -volume, surface area, specific surface area respectively. surface energies - liquid/vapour, liquid/solid, solid/vapour respectively (Nm-1) effective angle of friction voidage (volume fraction fluid) density (kg m-3) bulk, particle, skeletal densities respectively (kg m-3) variance of a distribution major consolidating stress shear stress
φw φ θ μk
CHAPTER 2 wall angle of friction angle of internal friction contact angle kth moment of a distribution
CHAPTER 3 WETTING, NUCLEATION AND BINDER DISTRIBUTION In Chapter 1, we divided granulation rate processes into three classes: wetting and nucleation, consolidation and coalescence, and breakage and attrition. Chapters 3 to 5 address each of these classes in turn beginning with wetting and nucleation. The first stage in any wet granulation process is the distribution of the liquid binder through the feed powder. Two extremes can be considered: (1) The liquid drop size is large compared to unit particle size; and (2) The particle size is large compared to the drop size. When the drop size is larger than the particle size, wetting the powder with the liquid gives a distribution of seed granules or nuclei. The nucleation process can be divided into four stages (see figure 3.1): 1. 2. 3. 4.
Droplets are formed at the spray nozzle at some size distribution and frequency. Binder droplets impact on the powder surface. Drops may coalesce at the powder bed surface and increase the effective drop size. The drop spreads across the bed surface and penetrates into the bed by capillary action to give a loosely packed nuclei granule. Shear forces within the bed may break up large wet clumps and nucleate into smaller entities.
These processes combine to define the nuclei size distribution produced as the powder passes through the spray zone of the granulator. When the drop size is small compared to the unit particle size, the liquid will coat the particles. The coating is produced by collision between the drop and the particle followed by spreading of the liquid over the particle surface. If the particle is porous, then liquid will also suck into the pores by capillary action (see figure 3.2). The wetting dynamics control the distribution of coating material which has a strong influence on the later stages of growth. The initial wetting and liquid distribution to produce nuclei or coat particles is important for a variety of reasons: • • • •
poor wetting leads to very broad nuclei size distributions and in extreme cases a mixture of overwet and ungranulated material. often the granulation retains a memory of the nucleation stage with broad nuclei size distributions leading to broad granule size distributions. preferential distribution of liquid between individual ingredients can cause component segregation with granule size. Wetting phenomena also influence downstream granule processes such as drying and redispersion in fluids.
Both the rate and extent of wetting are important for understanding nucleation and binder distribution. 37
There are relatively few studies in the literature on nucleation and wetting phenomena. Table 3.1 summarises some of the key experimental studies. Wetting and binder distribution have been variously blamed for changes in granule mean size, breadth of the granule size distribution, defluidisation and the presence of large clumps or agglomerates. Many variables, both formulation properties and process parameters, have been found to influence the quality of nucleation. In many cases, the experimental data are difficult to interpret because nucleation, growth and perhaps breakage are occurring simultaneously. One thing is clear, however. Poor nucleation and binder distribution almost always leads to poor control of granule properties with broad granule size distributions, possible wet quenching in fluid beds and clump formation in mixers and tumbling granulators.
Droplet Droplet Binder Binder coalescence dispersion formation dispersion & overlap by wetting & by capillary mechanical penetration mixing
Powder bed Figure 3.1. Nucleation during granulation offin e particles
L iq uid Drop
L iqu id A bsorbt ion into Pore s
Figure 3.2. Wetting and liquid spreading in systems where the particles are larger than the droplets
WETTING, NUCLEATION AND BINDER DISTRIBUTION
Table 3.1. Summary of research into wetting and granulation (Hapgood, 2000)
Worker Schæfer and Wørts (1978) Schaafsma et al (1999) Waldie (1991) Watano et al (1994) Holm et al. (1983, 1984) Aulton and Banks (1979) Gluba et al (1990) Jaiyeoba and Spring (1980) Krycer and Pope (1983) Zajic and Buckton (1990) Rankell et al (1964)
Materials Lactose and maize starch powder with gelatine, PVP and MCC binders Lactose powder with water and 3-8% PVP solution binders Lactose and ballotini powders with water and 5% PVP solution Lactose and cornstarch with water
Equipment Fluid bed
Investigated Drop size
Packed bed in Drop size petrie dish Fluid bed Drop size
Hybrid fluid bed with agitator Lactose and calcium hydrogen High shear phosphate with water and 10-15% PVP mixer solution Lactose and salicylic acid powder with Fluid bed water Talcum, chalk, and kaolin powder Drum combinations with water Lactose, boric acid, kaolin, Fluid bed suphanilamide and salicylic acid powders with water. Paracetamol powder with HPMC, PVP Fluid bed and water Methycellulose powder with HPMC, Mixer PVP and water granulator Aluminium hydroxide and sucrose Fluid bed powder with water
Heim and Antkowiak (1989) Crooks and Schade (1978) Kristensen and Schæfer (1994)
Talc powder and water
5% phenylbutazone in lactose powder mix with 10% solution Lactose powder with PEG300 and PEG6000
Schæfer et al. (1992)
Lactose powder with PEG300 and PEG6000
Cartensen et al (1976) Kokubo et al (1996) Davies and Gloor (1971)
Lactose, sucrose and starch powder mix High shear with water Lactose-cornstarch-MCC with HPMC High speed mixer 3cP Lactose, cornstarch, magnesium stearate, Fluid bed gelatin and benzene powder with gelatin solution
Drop size, binder distribution Drop size, binder distribution and shear forces Contact angle Contact angle Contact angle
Spreading coefficients Spreading coefficients Binder addition rate, powder flux, spray zone Binder addition rate Binder addition rate Viscosity, binder dispersion, shear forces, Viscosity, binder dispersion, shear forces, powder flux Binder dispersion Powder flux Spray zone
In this chapter, we take a systematic approach to nucleation and binder distribution, starting by defining important powder surface properties and how they can be measured. We then quantify nucleation phenomena in terms of some controlling groups and discuss how wetting and nucleation problems can be identified and overcome by changes to process conditions or formulation properties.
3.1. Powder Surface Properties 3.1.1. Some Definitions Molecules at the surface of a phase lack near neighbours. This leads to an excess free energy associated with the surface, or surface energy. When a drop of liquid sits on a solid surface there are three surface (interfacial) energies to consider (see figure 3.3):
the liquid-solid interfacial energy γ sl the liquid-vapour interfacial energy γ lv
the solid-vapour interfacial energy γ sv
γ lv θ
Three-phase contact line
Figure 3.3. Contact angle on a powder surface, where γ sv , γ sl , γ lv , are the solid-vapor, solid-liquid, and liquid-vapor interfacial energies, and θ is the contact angle
Surface energy has units of Jm-2 (energy per unit area of surface). Surface energy is often also called surface tension, especially when referring to the liquid-vapour interfacial energy. If a drop is static on the solid surface, the angle the drop makes with the surface, its contact angle θ, is such that the horizontal components of the three surface energies
WETTING, NUCLEATION AND BINDER DISTRIBUTION
balance (see figure 3-3). The contact angle is a measure of the affinity of the fluid for the solid as given by the Young-Dupré equation:
γ sv − γ sl = γ lv cos θ
When the solid-vapor interfacial energy exceeds the solid-liquid energy, the fluid wets the solid with a contact angle less than 90°. In the limit of γ sv − γ sl ≥ γ lv , the contact angle equals 0° and the fluid spreads on the solid. The extent of wetting is controlled by the group γ lv cos θ which is referred to as adhesion tension. Work is required to create new surface. We can define the work of cohesion as the work required to separate a unit cross sectional area from itself and the work of adhesion as the work required to separate a unit area of cross section at the interface between two phases (see figure 3.4). The work of adhesion and cohesion can be written in terms of surface energies: Wcs = 2γ sv
Wcl = 2γ lv
Wa = γ sv + γ lv − γ sl = γ lv (1 + cos θ )
Workof cohesion for a solid
Wcs = 2γ sv
Workof cohesion for a liquid
Wcl = 2γ lv
Workof adhesion for aninterface
Wa = γ sv + γ lv − γ sl
Figure 3.4. Diagram showing cohesion and adhesion in solid and liquid systems (adapted from York (1995))
We should emphasise that surfaces are not homogeneous or pure (see figure 3.5). Both hydrophobic and hydrophilic sites may be present on the same particle, as well as ions and other adsorbed species eg. impurities and surfactants. To a first approximation, we can consider the total surface energy of the powder surface to be made up of a dispersive and a polar component:
γ sv = γ svP + γ svD
These components reflect the chemical character of the interface, with the polar component due to hydrogen bonding and other polar interactions and the dispersive component due to van der Waals interactions. The surface energy of the liquid binder can also be arbitrarily divided into polar and dispersion components. When solid and liquid surfaces are brought together, the dispersion and polar components of the two surface energies will interact to reduce the overall solid-liquid interfacial energy. Various models exist to predict this interaction quantitatively (York, 1995). The two most common models are the geometric mean and harmonic mean models:
γ sl = γ sv + γ lv − 2§¨ γ svD γ lvD + γ svP γ lvP ·¸ ©
§ γ svD γ lvD γ svP γ lvP + ¨γ D +γ D γ P +γ P lv sv lv © sv
γ sl = γ sv + γ lv − 4¨
¹ · ¸ ¸ ¹
Equations 3-1 and 3-4a can be combined to give the contact angle as a function of the polar and dispersive interactions between the powder and the binder eg. using the geometric mean: 2§¨ γ svD γ lvD + γ svP γ lvP ·¸ γ sv − γ sl © ¹ cos θ = = −1 + γ lv γ lv
These models are semi-empirical rather than fundamentally based. The polar interaction, in particular, is difficult to predict. In discussion below, we will use the geometric mean model (eqns. 3-4a and 3-5) but caution is advised. This is a brief summary of key surface properties. For more detailed discussion of powder surface properties, wetting and dispersion see Parfitt (1986) and Ayala (1985).
WETTING, NUCLEATION AND BINDER DISTRIBUTION
~, : : fctiv~ excipients
Figure 3.5. The heterogeneous nature ofpowder-liquid inteifaces
3.1.2. Methods of Measurement There is no single ideal method to characterise the surface properties of powders. The four possible approaches are summarised in Table 3.2. Each ofthe methods is discussed below.
Sessile Drop Studies. Sessile drop studies to measure contact angle can be performed on powder compacts in the same way as on planar surfaces. A drop is placed on the compact surface and the contact angle measured in one of three ways: 1) 2) 3)
direct measurement of the contact angle from the tangent to the air-binder interface, solution of the Laplace-Young equation involving the contact angle as a boundary condition, or indirect calculations of the contact angle from measurements of drop height.
If the compact is dry, the drop will simultaneously spread and sink into the compact. Therefore, to measure static contact angle, the compact must first be saturated with fluid. However, experiments with dry compacts to give useful dynamic measurements may be made through a computer imaging goniometer as depicted in figure 3.6 (Pan et at., 1995). Figure 3.7 gives an example of dynamics of drop penetration and spreading on a compact of herbicide granules. The short time dynamic data is found to be more sensitive to the differences between the different batches than the longer time data and that spreading velocity decreases with time. These dynamics are affected by the rate of ingredient dissolution and adsorption/desorption kinetics of surface active agents. The main weakness in sessile drop techniques for powders is that it is very difficult to get reproducible data. Results are extremely sensitive to how the powder compact is prepared, especially to porosity at the compact surface. Preparing the compact may also break particles or granules, changing their surface properties.
CHAPTER 3 Table 3.2. Methods a/Characterizing Powder SUljace Properties
~ ~n&I-tertjes, GU11 Eng.
Sci. , 3), JJ3
Raecf r:erItratim ~ Jrigtt (T \dune
BfEn'll.'ei: Pafill (ed.),llip:rsim ifJtMclo:s in Lipids, 19?6 WIsIb.m, Rl)'$. Rev., 17, m (I92l} &reI1 &0iteJtd; Ird. Eng. Or!m, 19, rm (1927).
.RntIaim tine Srlrrert teigtt Gitiall sdid ~fa:e emgy distrib1im
Bfm'mS R A~a, RlD1le;i (rem Erg, Qmgie M:l101UDv. (lS8S). RmtamIua d., Gikids & .'i ~ 127 19)1.
Rtfereliial adnJrim \Vith pm ~
ElectrdinD1), a slurry or over-wetted mass will be formed. 1.0E+0 Crumb
St def = ρ U 2/ 2Y (-)
Tardos et al . (1998)
Induction Nucleation Steady Growth Rapid Growth
Steady Growth Iron Ore in Drum
1.0E-2 Nucleation Region
Ballotini & Water in Drum
1.0E-3 Ballotini & Glycerol in Drum
Chalcopyrite in Drum
Pore Saturation (-) Figure 4.26. Growth regime map with data for granulation of a wide range of materials
The growth regime map is shown in figure 4.26 (Iveson et al., 2001). The map shows a wide range of literature data for drum granulation, including data from figures 4.24 and 4.25. The data fits the regime map reasonably well. The transition from nucleation to
CONSOLIDATION, COALESCENCE AND GROWTH
steady or induction growth occurred at pore saturations between 80% and 90%. Rapid growth occurred for all pore saturations greater than 100 %. The boundary between induction and steady growth occurred at Stdef between 0.001 and 0.003. The steady growth results all lie well below the steady-crumb regime boundary of 0.2 measured by Tardos et al. (1997). Figure 4.27 shows the regime map with the mixer experimental results added. In many cases mixer results do not fit the regime map as set for drum granulation. The most likely reason for the failure of the regime map to predict the granulation behaviour in the mixers is that, since Stdef is proportional to impact velocity squared, any errors in estimating typical impact velocity will be greatly magnified. It is difficult to know what characteristic speed to use to characterise a mixer granulator. In a horizontal-axis, high shear Lödige mixer growth rate is sensitive to chopper speed but not to impeller (plough share) speed (Menon, 1996). The chopper tip-speed was chosen as the collision velocity to use in calculating Stdef. when analysing the data of Hoornaert et al. (1998). However, these observations are not universal to all high shear mixers. In vertical axis mixers, several studies showed no effect of chopper speed on growth eg. (Knight (1993). For vertical axis mixers, collision velocity is probably closely related to impellor tip speed. 1.0E+1 Iron Ore in Mixer
St def = ρ U 2/ 2Y (-)
Na2SO4 in Mixer
Tardos et al . (1998)
Crumb Steady Growth
1.0E-1 Ballotini & PEG in Mixer
Induction Nucleation Steady Growth
Iron Ore in Drum
1.0E-2 Nucleation Region 1.0E-3
Ballotini & Water in Drum Chalcopyrite in Drum
Ballotini & Glycerol in Drum
Pore Saturation (-) Figure 4.27. Stdef vs pore saturation for drum and mixer granulation experiments with glass ballotini, iron ore, chalcopyrite and sodium sulphate powders (Iveson et al., 2000).
In summary, the regime map is a useful tool for predicting granule growth behaviour in tumbling granulators. There is still some way to go to extend it fully to the more complex behaviour in mixers.
he growth regime will influence profoundly approaches to scale up and control. If a powder-binder mixture lies in the induction growth region (strong, non-deformable granules), then provided its induction time is not exceeded, it will never grow rapidly. The granule size distribution will be controlled by the nucleation conditions. Layering growth could be promoted by spraying binder onto the surface of pre-existing granules, whereas smaller granules could be formed by spraying the binder onto the fresh feed to promote nucleation. Therefore the product size distribution will be strongly influenced by the positioning of the liquid nozzle(s) and powder feed, liquid droplet size distribution, powder wetting characteristics and the flow and mixing of material in the granulator. This kind of formulation will be relatively easy to scale with respect to granule size distribution since there is a long period of little growth. However, care must be taken that the process agitation intensity does not increase significantly during scale up (eg. from a small to large pan). Such an increase may shift the formulation’s behaviour from the induction region to the steady growth region, in which case scale up will be much more difficult. The growth behaviour of powder-binder mixtures in the steady growth region (weak, easily deformable granules) is dominated by coalescence, not layering or nucleation. The rate of coalescence is very sensitive to binder content and scale of operation because these variables both affect the granule deformability. This type of formulation is difficult to scale-up with respect to granule size distribution. Granule size is controlled by the rate of liquid addition and is also a strong function of the residence time. On the other hand, porosity will be insensitive to residence time since granules will quickly reach their minimum porosity.
4.6. Control of Growth and Consolidation for Particle Design The granule mean size, the breadth of the granule size distribution and the granule porosity (density) are all influenced by the way granules grow and consolidate. This section summarises the effect of process parameters and formulation properties on growth and consolidation behaviour, and hence granule attributes, based on the fundamental understanding of granule growth we have developed.
4.6.1. Elastic Granule Systems Systems that can be treated as elastic (non-deformable) are: • Granulation with simultaneous drying (fluidised beds, spouted beds, etc.) • Systems where the maximum feed particle size is much larger than the spray drops (coating/layering processes, processes where feed includes recycled granules of order of the size of the desired product granules) These systems are described by the Stokes regime analysis. It is important to establish in which regime the system in operating (non-inertial, inertial, coating) and whether the system traverses more than one regime during granulation. The effect of process parameters and formulation properties is encapsulated in the dimensionless groups Stv and St*.
CONSOLIDATION, COALESCENCE AND GROWTH
4.6.2. Deformable Granule Systems Deformable granule systems have powder feeds wet by a spray whose drop size is large compared to the feed powder and where simultaneous drying does not occur. These systems are characterised primarily by the dimensionless groups smax and Stdef , with Stv having a secondary effect. The granulation regime map (figure 4.26) can be used to establish the growth regime and decide on scale up and control strategies. Effect of formulation properties The single most important formulation property is the liquid content. As liquid content increases, the granulation regime moves from nuclei only through steady growth or induction time to rapid growth and slurry formation. In the nuclei regime, slow controlled growth can be achieved by successive powder layering. The operating window for controlled growth by coalescence is often very small with growth rate and granule size increasing exponentially with liquid saturation (see figure 4.28) (Ritala et al., 1988, Litster and Waters, 1986). Thus, granule size is very sensitive to liquid content in this region. The effect of other formulation properties should be viewed in terms of their effect on granule yield stress. Increasing binder viscosity increases granule dynamic strength and hence decreases Stdef (see section 4.1.2). This decreases the rate of granule consolidation and increases the equilibrium granule porosity generally leading to a more porous granule (section 4.2). Increasing viscosity can move a system from the crumb region to steady growth (Keningley et al., 1997) or from steady growth to induction behaviour (Knight et al., 1998, see also figure 4.26). So the effect on growth rate and final granule size depends on the growth regime and the residence time in the granulator. This is emphasised by figure 4.29. In high shear mixer granulation, granules grew faster with the lower viscosity binder but reached a smaller final (equilibrium) granule size. Increasing liquid viscosity or decreasing particle size both increase granule dynamic yield stress but have variable effects on minimum porosity (Iveson et al., 1996, Iveson and Litster, 1998a, Iveson and Litster, 1998b). Hence, increasing binder viscosity and decreasing particle size will decrease Stdef and should shift a formulation’s behaviour towards the bottom of the regime map ie. from crumb to steady growth; and from steady growth to induction time behaviour.
Figure 4.28. Effect of moisture as a percentage of granule saturation on mean granule diameter. Granulation of calcium hydrogen phosphate with aqueous binder solutions in a Fielder PMAT 25 VG high-shear mixer (Ritala et al., 1988)
Results in the literature support these predictions. Capes and Danckwerts (1965) found that decreasing particle size shifted behaviour from the crumb into the steady growth region. The increasing frequency of induction time behaviour with decreasing particle size can be seen by surveying the existing literature. Workers who studied coarse, narrowlysized silica sands, did not observe induction behaviour (eg. Capes and Danckwerts, 1965; Newitt and Conway-Jones, 1958). Linkson et al. (1973) saw induction times of up to 200 revolutions with widely-sized, 43 μm silica sands. Induction times of over 1000 revolutions have been frequently observed with finely ground limestone powders (0.71 m2/g) and hematite ores (0.295 m2/g) (Kapur, 1978; Sastry et al., 1977).
CONSOLIDATION, COALESCENCE AND GROWTH
(b) Figure 4.29. Granule diameter as a function of time for high-shear mixer granulation. (a) 10-liter vertical high-shear melt granulation of lactose with liquid loading of 15 wt % binder and impeller speed of 1400 rpm for two different viscosity grades of polyethylene glycol binders. (Schaefer et al., 1990). (b) 10-liter vertical high-shear mixer granulation of dicalcium phosphate with 15 wt % binder solution of PVP/PVA Kollidon® VA64, liquid loading of 16.8 wt % and chopper speed of 1000 rpm for varying impeller speed. (Schaefer et al., 52(9), 1990).
Decreasing binder surface tension has been found to decrease both dynamic yield stress and the extent of granule consolidation (Iveson and Litster, 1998a; Iveson and Litster, 1998b). Hence, lowering binder surface tension will increase Stdef and decrease smax. This will shift a formulation’s behaviour towards the top-left of the regime map ie. from induction to steady growth; and from steady growth to crumb or nucleation behaviour. Capes and Danckwerts (1965) found that lowering binder surface tension did shift a material into the crumb region. However, no studies have been done to test whether lowering binder surface tension can shift a material’s behaviour from induction to steady growth. Effect of process parameters Increasing process agitation intensity will increase the typical impact velocity and hence increase the deformation number. The consolidation models of Ouchiyama and Tanaka (1980) and Ennis et al. (1991) both predict that granule consolidation will increase with increasing frequency and energy of impacts. This has been confirmed experimentally in tumbling pans, high-shear mixers and agitated fluidised beds where it was found that increasing pan or impeller speed increased the initial rate of consolidation (Ouchiyama and Tanaka, 1980; Ritala et al., 1986; Watano et al., 1995). Likewise, the porosities of granules made in high-shear mixers are generally much lower than those made in tumbling drums and pans (eg. 20 to 40% measured by Kristensen et al. (1985) compared with 40 to 50% measured by Kapur and Fuerstenau (1969)). Hence, increasing process agitation intensity will increase the extent of granule consolidation and hence increase the maximum pore saturation. Therefore, increasing agitation intensity should shift a system’s behaviour towards the top-right of the proposed growth regime map ie. from nucleation to steady or induction growth; from induction to steady or rapid growth; and from steady growth to crumb, rapid or over-wetted growth (see Figure 4.31). There is some evidence for this in the literature. Poskart (1988) used a tumbling drum mounted on a spinning arm and found that increasing the centrifugal force from 1 to 10-50 g significantly increased the product density. At 50 g, destructive forces dominated and very few pellets were formed (“crumb” region). The process also became very sensitive to binder content and could easily “sludge” (ie. form an over-wetted mass or slurry). Similarly, Keningley et al. (1997) found that increasing impeller speed shifted a material’s behaviour from the steady growth to the crumb region (their so-called “paste” region). However, no work is currently available to confirm whether increasing agitation intensity will also shift a material’s behaviour from induction to steady growth as predicted by this regime map. Table 4.3 gives a quick reference summary of the role of formulation properties and process parameters in controlling growth and consolidation.
CONSOLIDATION, COALESCENCE AND GROWTH Table 4.3. Controlling Growth and Consolidation in Granulation Processes Typical changes in material or operating variables which maximize growth and consolidation Rate of growth (low deformability): Increase rate of nuclei formation
Appropriate routes to alter variable through formulation changes Improve wetting properties. (See "Wetting" subsection.) Increase binder distribution.
Increase collision frequency
Appropriate routes to alter variable through process changes Increase spray rate and number of drops. Increase mixer impeller or drum rotation speed or fluidbed gas velocity. Increase batch time or lower feed rate.
Increase residence time Rate of growth (high deformability): Decrease binder viscosity
Decrease binder concentration or change binder. Decrease any diluents and polymers which act as thickeners.
Increase agitation intensity Increase particle density Increase rate of nuclei formation, collision frequency and residence time, as above for low deformability systems Extent of growth: Increase binder viscosity
Increase mixer impeller or drum rotation speed or fluidbed gas velocity.
Increase binder concentration, change binder, or add diluents and polymers as thickeners.
Decrease agitation intensity
Decrease particle density Increase liquid loading Rate of consolidation: Decrease binder viscosity Increase agitation intensity Increase particle density Increase particle size
Decrease operating temperature for systems with simultaneous drying. Otherwise increase temperature.
Increase operating temperature for systems with simultaneous drying. Otherwise decrease temperature. Decrease mixer impeller or drum rotation speed or fluidbed gas velocity. Extent observed to increase linearly with moisture.
As above for high deformability systems. Particle size and friction strongly interact with binder viscosity to control consolidation. Feed particle size may be increased and fine tail of distribution removed.
As above for high deformability systems. In addition, increase compaction forces by increasing bed weight, or altering mixer impeller or fluid-bed distributor plate design. Size is controlled in milling and particle formation.
ography Adams, M.J., Thornton, C. and Lian, G. (1994). 1st Int. Part. Tech. Forum, vol 1, Denver, Aug.17-19, 220. Adetayo, A.A., Litster, J.D. and Desai, M. (1993). Chem. Eng. Sci., 48, 3951. Adetayo, A.A., J.D. Litster, S.E. Pratsinis and B.J. Ennis (1995). Powder Technol., 82, 37. Capes, C.E. and Danckwerts, P.V. (1965). Trans. I. Chem. Eng., 43, 116. Capes, C.E. (1980). Particle Size Enlargement, Elsevier. Ennis, B.J., Tardos, G.I. and Pfeffer, R. (1991). Powder Technol., 65, 257. Holm, P., Schaefer, T. and Kristensen, H.G. (1985). Powder Technol., 43, 213. Hoornaert, F., Meesters, G., Pratsinis, S. and Scarlett, B. (1994). 1st Int. Part. Tech. Forum, Denver, 278. Iveson, S.M., Litster, J.D. and Ennis, B.J. (1996) Powder Technol., 88, 15. Iveson, S.M. and Litster, J.D. (1998a). Powder Technol., 99, 234. Iveson, S.M. and Litster, J. D. (1998b). Powder Technol., 99, 243. Iveson, S.M. and Litster, J.D. AIChE., 44 (7), 1510 (1998c). Iveson, S.M. and N.W. Page (1998). Proc. CHEMECA '98, Port Douglas, Queensland, Australia, 28-30 September., paper 259. Iveson, S.M., Beathe, J.A. and Page, N.W. (2002). Powder Technology, 127, 149-161. Iveson, S.M., Wauters, P.A.L., Forrest, S., Litster, J.D., Meesters, G.M.H, Scarlett, B., (2001). Powder Technology, 117, 83-87. Johnson, K.L. (1987). Contact mechanics. Cambridge University Press. Kapur, P.C. and Fuerstenau, D.W. (1968). I&EC Proc. Des. Dev., 8, 56. Kapur, P.C. (1978). Advances in Chemical Engineering, 10, 55. Keningley, S.T., Knight, P.C. and Marson, A.D. (1997). Powder Technol., 91, 95. Knight, P.C., Instone, T., Pearson, J.M.K. and Hounslow, M.J. (1998). Powder Technol., 97, 246. Kristensen, H.G., Holm, P. and Schaefer, T. (1985). Powder Technol.,, 44, 227. Kristensen, H.G., Holm, P. and Schaefer, T. (1985). Powder Technol., 44, 239. Linkson, P.B., Glastonbury, J.R. and Duffy, G.J. (1973). Trans. Instn. Chem. Engrs., 51, 251. Litster, J. D., Waters, A.G. and Nicol, S.K. (1986). Trans. ISIJ, 26 (12), 1036. Liu, L.X. and Litster, J.D. (1993). Powder Technol., 74, 215. Liu, L.X., Litster, J.D. Iveson, S.M. and Ennis, B.J. (2000). AIChE J., 46, No.3, 529. Newitt, D.M. and Conway-Jones, J.M. (1958). Trans. I. Chem. Eng., 36, 422. Nienow, A.W. and Rowe, P.N. (1985). Particle growth and coating in gas-fluidised beds, in: J. Davidson (Ed.), Fluidization, Academic Press, London. Ouchiyama, N. and Tanaka, T. (1975). I&EC process Des. Dev., 14, 286. Ouchiyama, N. and Tanaka, T. (1980). Ind. Eng. Chem. Fundam., 19, 555. Poskart, M.B. (1988). Evaluation of a New Pelletiser BS Thesis, Dept of Chem. Eng., Univ. of Queensland, Australia. Ritala, M., Jungersen, O., Holm, P., Schaefer, T. and Kristensen, H.G. (1986). Drug Dev. Ind. Pharm., 12, 1685. Ritala, M., Holm, P., Schaefer, T. and Kristensen, H.G. (1988). Drug Dev. Ind. Pharm., 14, 1041. Rumpf, H. (1962). The Strength of Granules, and Agglomerates, in Agglomeration, W.A. Knepper, ed., Interscience, New York, p. 379.
CONSOLIDATION, COALESCENCE AND GROWTH
Sastry, K.V.S. and Feurstenau, D.W. (1975). Int. J. Miner. Process, 2, 187. Sastry, K.V.S., S.C. Panigraphy, and D.W. Fuerstenau (1977). Trans. Soc. Mining Engineers, 262, 325. Schaefer, T. and Worts, O. (1977) Archiv for Pharaci og Chemi 5, 51. Schaefer, T. Holm, P. and Kristensen, H. G. (1990). Pharm. Ind., 52 (9), 1147. Schaefer, T., Holm, P. and Kristensen, H. G. (1990). Drug Dev. & Ind. Pharm., 16(8), 1249. Schubert, H. (1975). Powder Technol., 11, 107. Tardos, G.I., Khan, M.I. and Mort, P.R. (1997). Powder Technol., 94, 245. Waldie, B. (1991). Chem. Eng. Sci., 46 (11) 2871. Watano, S., Sato, Y., Miyanami, K., Murakami, T., Nagami, N., Ito, Y., Kamata, T. and Oda, N. (1995). Chem. Pharm. Bull., 43, 1217. Wauters, P.A.L., van de Water, R., Litster, J.D., Meeters, G.M.H., Scarlett, B. (2001). Powder Technology, 124.
4.8. Nomenclature a Ao A1 Ca dp db dg, D e g h, hb ha Ke m N(t) n(v,t) s Stv St* Y u Uc ub w ȕ(u,v) İmin İb İ
particle radius (m) initial area of the sample (m2) the deformed contact area after impact (m2) Capillary number (-) particle size (m) volume equivalent bubble size (m) granule size (m) coefficient of restitution (-) gravitational acceleration (m s-2) liquid layer thickness (m) height of surface asperities (m) compaction rate (-) particle mass (kg) total number of granules at time t number density of granules of size v at time t liquid saturation of pores (-) viscous Stokes number critical Stokes number granule dynamic yield stress ((N m-2) velocity (m s-1) collision velocity (m s-1) bubble rise velocity (m s-1) effect mean particle mass during a collision (kg) coalescence rate constant for collisions between granules of volumes u and v minimum granule porosity (-) bed voidage (-) granule porosity (-)
į ȡg ȡl ȡp ıD ıT Ȧ
CHAPTER 4 surface tension (N m) granule deformation (m) granule density (kg m-3) liquid density (kg m-3) particle density (kg m-3) peak flow stress (N m-2) granule static tensile strength (N m-2) viscosity (Pa s) rotational speed (sec-1)
CHAPTER 5 BREAKAGE AND ATTRITION This chapter considers the last of the three classes of granulation processes that control granule attributes – breakage and attrition. There are really two separate phenomena to consider here: 1. 2.
Breakage of wet granules in the granulator; and Attrition or fracture of dried granules in the granulator, drier or in subsequent handling.
Breakage of wet granules will influence and may control the final granule size distribution, especially in high shear granulators. In some circumstances, breakage can be used to limit the maximum granule size or to help distribute a viscous binder. Attrition of dry granules leads to the generation of dusty fines. As the aim of most granulation processes is to remove fines, this is generally a disastrous situation to be avoided. In this chapter, breakage of wet and dry granules are treated separately. We take the same approach as in chapter 3 and 4. Where possible, key formulation and granule properties are defined and the controlling groups or equations for the breakage processes are developed. 5.1. Breakage of Wet Granules 5.1.1. Experimental Observations Few investigators have described or studied wet granule breakage in granulation processes. Some preferential growth mechanisms in tumbling granulation may involve attrition or breakage of weak granules (crushing and layering, abrasion transfer) (Sastry and Feurstenau, 1975). However, breakage is much more likely in higher intensity mixer and hybrid granulators. The limited work on wet granule breakage focuses on these processes. Several studies show an increase in agitation intensity (increased impeller speed) reduces the final granule mean size in granulation experiments (Knight et al., 2000; Holm et al., 1983; Watano et al., 1995). For example, figure 5.1 shows median granule size from three scales of agitated fluid bed granulator decreases with increasing agitator tip speed. However, reduction in product size with increased agitation could also be explained by a reduction in the maximum granule size for coalescence (see chapter 4). So changes to granule size distribution, on their own, are insufficient evidence for wet granule breakage as a key mechanism for controlling granule properties. However, wet granule breakage has been identified clearly in high shear mixer experiments by other means. Ramaker and co-workers (1998, Vonk et al., 1997) and Pearson et al. (1998) both used coloured tracer granules or liquid to identify breakage of wet granules. Pearson et al. added narrow size fractions of well formed tracer granules part way through a batch high shear granulation. Some of the tracer granules were broken, leaving coloured tracer fragments in smaller granule size fractions. Large tracer granules (>1mm) were more likely to be broken than smaller granules (figure 5.2). Knight et al (2000) showed mean granule size decreased after impeller speed was suddenly increased 121
ugh a batch high shear mixer experiment. This was attributed to granule breakage. Ramaker and co-workers added a coloured liquid at the start of the granulation process and observed the dispersion of the dye through a process of “destructive nucleation” where loosely bonded nuclei are broken down into smaller fragments via attrition or fragmentation (figure 5.3). The initial weak nuclei were quite large in these experiments (5mm diameter). We can view this process as simply a subset of breakage processes in the granulator. In fact, all binder distribution in the “mechanical dispersion” (chapter 3) is essentially a breakage process and should be treated as such. In summary, wet granule breakage is potentially an important process affecting binder distribution and granule size in high intensity processes. Therefore it is important to establish the conditions under which breakage will occur.
Figure 5.1. Effect of impeller speed on median particle size in an agitated fluid bed granulator (Tardos et al., 1997)
BREAKAGE AND ATTRITION
Figure 5.2. Breakage of tracer granules in high shear mixers: Effect of tracer granule size on mass fraction of unbroken granules (Pearson et al., 1998)
Figure 5.3. The destructive nucleation mechanism proposed by the Groningen group (Vonk et al., 1997)
CHAPTER 5 cting Conditions for Breakage
There is very little quantitative theory or modelling available to predict conditions for breakage, or the effect of formulation properties on wet granule breakage. We present a criteria for breakage based on the concepts proposed by Tardos et al. (1997a,b) combined with the understanding of granule behaviour developed in chapter 4. Consider that a granule will break if the applied kinetic energy during an impact exceeds the energy required for breakage. This analysis leads to a Stokes deformation number criteria for breakage: * St def > St def
* is the where Stdef is the Stokes deformation number as defined by eqn.4-14 and St def
critical value of Stokes number that must be exceeded for breakage to occur. There are strong analogies to the development of the Stokes deformation number for granule deformation and growth (eqn. 4-4). It is likely the critical value for breakage will be greater than that for coalescence as granules may deform plastically at the impact point without breakage of the granule. Even this is an oversimplification. A purely plastic granule will smear rather than break when its yield stress is exceeded. At high impeller speeds such materials will coat the granulator wall or form a paste. Semi- brittle granules will break at high impact velocity giving a maximum stable granule size or a weak crumb. Thus, considerable information about the granule mechanical properties is needed to predict their behaviour. Note this yield behaviour should be measured at strain rates similar to those during impact in the granulator, not in static mechanical tests. Note that the original work of Tardos et al. (1997a,b) proposed a more loosely defined characteristic stress than the dynamic yield stress in eqn.4-4 and considered breakage of granules by shear rather than impact. They postulate the granule will behave under shear as a Herchel-Buckley fluid ie.
τ (γ ) = τ y + kγ n
Two simplifications were considered, neglecting either the apparent viscosity ( τ (γ ) = τ y ) or the yield stress ( τ (γ ) = kγ n ). In either case, the model predicts granules above a maximum size will break and this size is decreased with increasing shear rate. Tardos and co-workers measured granule deformation and break up under shear in a novel constant shear fluidised bed granulator. Granules first elongated under shear and then broke at a Stokes deformation number of approximately 0.2. Tardos’s work was pioneering. However, in mixer granulators, granules may break on impact with the impeller or chopper, rather than in shear. In this case, the appropriate “critical stress” should be the dynamic yield stress measured under high strain rate conditions, as discussed in chapter 4. Kenningley et al. (1997) developed a relationship for breakage (crumb, paste) or survival of granules in high shear mixer granulation by equating kinetic energy of impact to energy absorbed by plastic deformation of granules The granule yield strength was
BREAKAGE AND ATTRITION
assumed to be due to viscous pressure loss for fluid flow between particles by KozenyCarman equation. The amount of strain (εm) was given by:
ε m2 =
1 ε 3 ρud 3, 2 1 ε3 = St v 540 (1 − ε )2 μ 540 (1 − ε )2
where d3,2 is the Sauter mean size of the granules’ constituent particles. Increasing Stv increases the amount of impact deformation. Above a critical value of εm (taken as 0.10 by Kenningley et al., 1997), granules will break. They showed reasonable agreement with their experimental data (see figure 5-4).
Figure 5.4. Variation of binder viscosity required to form granules with size of constituent particle (Source: Kenningley, et al. 1997).
Although, the fundamental basis for predicting breakage is incomplete, we can still use our limited knowledge for scale up. For breakage, the appropriate velocity for the Stokes deformation number is the maximum collision velocity a granule can experience with another granule or with part of the granulator equipment. For mixer granulators, this is clearly the impeller tip speed. Eqns 5-1 and 5-3 suggest breakage will increase with increasing tip speed. Figure 5-1 shows that the relationship between tip speed and granule mean size was the same for three different scales of agitated fluidised bed granulators, as we would expect if granule size were controlled by breakage processes.
5.1.3. Controlling Granule Attributes through Breakage Controlling wet granule breakage gives the opportunity to give a narrow granule size distribution by growing granules up to a breakage limit (Tardos et al., 1997a; Knight et al.,
Mort and Tardos, 1999; Ramaker et al, 1998). This has been the driving force in the development of some newer granulator designs (Watano et al., 1995; Dencs and Ormos, 1993). It is important to note that size distribution control will also depend on the impact velocity distribution and turnover of granules through the high impact region (impeller or chopper). Granulators with broad impact velocity distributions and small, uncontrolled turnover through the high impact region are unlikely to ever yield narrow granule size distributions. Controlling granule breakage for particle design is discussed further in section 5.3.
5.2. Attrition and Fracture of Dry Granules Most granulation processes involve drying granules either simultaneously (fluidised bed and spouted bed granulators) or immediately after granulation in a separate drier. Attrition or fracture of the granules during granulation, drying or subsequent handling is generally undesirable. Therefore understanding the attrition processes and parameters which effect them are important. There is limited fundamental work on the fracture of dry granules but we can draw on more general understanding of the fracture of brittle and semi-brittle materials. Adams and Briscoe (1987) provide good background in this area. 5.2.1. Fracture Properties of Dry Granules From the point of view of breakage, we can consider a dry granule as a non-uniform physical composite rather than an agglomerate of primary particles. The composite possesses certain macroscopic mechanical properties including a yield stress. Instead of porosity, we see an inherent distribution of cracks and flaws. Dry granules fail in brittle or semi-brittle fashion i.e. they fail in tension by the propogation of pre-existing cracks which concentrate stress. Thus, the fracture stress may be much less than the inherent tensile strength of bonds between particles in the granule. Consider a brittle material failing by crack propogation (figure 5.5). The tensile stress concentrates near the crack tip and is much higher than the applied stress. The fracture toughness of the granule Kc defines the elastic stress field in the granule ahead of the propogating crack and is given by (Lawn, 1975): K c = Yσ f πc
A simple elastic fracture model predicts an infinite stress at the crack tip. The elastic stress cannot exceed the yield stress of the material, leading to local yielding near the crack tip. To apply the simple framework of linear elastic fracture mechanics, the process zone size can be considered as an effective increase in crack length δc (Irwin, 1957). Fracture toughness is then given by: K c = Yσ f π (c + δc) with δc ~ r p
BREAKAGE AND ATTRITION
The process zone size is a measure of the yield stress or plasticity of the material in comparison to its brittleness. Yielding within the process zone may take place either plastically or by diffuse microcracking, depending on the brittleness of the material. Crack propogation can also be viewed from an energy perspective. The critical strain energy release rate Gc due to crack propogation must exceed the rate of creation of surface energy for the crack to propogate (Griffith, 1920). Gc is the energy equivalent of fracture toughness. They are related by: Gc =
Y 2σ 2f πc E
K c2 E
These properties, together with the flaw distribution in the material dictate how it will break. Therefore, characterising these properties of a granule is an important prerequisite to determining its attrition and fracture behaviour.
Figure 5.5. Fracture of a brittle material by crack propagation
5.2.2. Measurement of Fracture Properties Granule breakage and attrition is an area in which rituals abound. However, ranking of granule breakage resistance by ad hoc tests may be test specific, and in the worst case differ from the ranking under actual conditions. Instead, standardised mechanical tests should be employed to minimise the effect of flaw and loading conditions under well defined geometries of internal stress, as described below. To measure fracture properties reproducibly, very specific test geometry must be used since it is necessary to know the stress distribution at predefined induced cracks of known length. Three traditional methods are the three point bend test, indentation fracture testing and Hertzian contact compression between two spheres. Figure 5.6 shows a schematic of a three point bend test. Firstly, formulation powder is premixed with liquid binder to the expected level for granulation. A series of bars, each of known crack length, are formed by compacting the moist premix in moulds containing a razor notch. The bars are then dried. The force displacement of the bars is then measured up to fracture in a 3 point bend test. Kc and δc are then determined by regressing the measured fracture stress against the known crack length (eqn.5-4). Figure 5.7 shows an example of the force displacement curve from a three point bend test on an agglomerate bar. The main difficulty with the three point bend test for agglomerated materials is in the preparation of the bars. Results are sensitive to the way the bars are made and the bar structure will not match exactly the structure of a granule formed in, for example, a mixer granulator. Nevertheless, the technique been used successfully to study fundamentals of granule fracture, as well as for process troubleshooting (Seville and Ennis, 1990; Ennis and Sunshine, 1993).
Figure 5.6. Schematic of 3 point bend test apparatus
BREAKAGE AND ATTRITION
Figure 5.7. Three point bend test results: Typical force displacement curve for semi-stable fracture
Fracture toughness and hardness can also be determined from indentation tests (Johansonn and Ennis, 1994). An indent is made in a granule with known maximum force F (figure 5.8). The hardness is determined from the area of the residual plastic impression and the fracture toughness from the length of the cracks propogating from the indent as a function of load:
Kc = β
E F F and H ~ H c3/ 2 A
Figure 5.9 shows the plastic impression and radiating cracks from an indentation in an alumina catalyst particle. For this technique to be useful for agglomerates, the indentation must be large compared to the size of the feed particles but small compared to the size of the product granule. Careful presentation of the granule to the indentor is also important. This test does have the advantage that measurements can be made on real granules. The heterogenous nature of agglomerates means they exhibit more scatter in mechanical testing than some other materials and consistent sample preparation is very important. Nevertheless, the key advantage of these tests remains that fundamental properties are measured and the influence of natural flaw distribution on the results is small. Table 5-1 compares typical fracture properties of agglomerated materials. Fracture toughness Kc is seen to range from 0.01 to 0.06 MPa.m1/2, less than that typical for polymers and ceramics, presumably due to the high agglomerate voidage. Critical strain energy release rates Gc from 1 to 200 J/m2, typical for ceramics but less than that for polymers. Process zone sizes įc are seen to be large and of the order of 0.1-1 mm, values
for polymers. Ceramics on the other hand typically have process zone sizes less than 1 f.lm. Critical displacements required for fracture may be estimated by the ratio Gj E, which is an indication of the brittleness of the material. This value was of the order of 10- 7 - 10-8 mm for polymer-glass agglomerates, similar to polymers, and of the order of 10-9 mm for herbicide bars, similar to ceramics. In summary, granulated materials behave similar to brittle ceramics which have small critical displacements and yield strains but also similar to ductile polymers which have large process or plastic zone sizes.
Figure 5.8. Schematic of indentation test for single particle or granules
Figure 5.9. Indentation in an alumina catalyst particle showing propogation ofcracks
BREAKAGE AND ATTRITION
Table 5.1 Fracture Properties of Agglomerate Materials (Ennis and Sunshine, 1993) Material Bladex 60™† Bladex 90™† Glean™† Glean Aged™† CMC-Na(M)‡ Klucel GF‡ PVP 360K‡ CMC 2% 1kN‡ CMC 2% 5kN‡ CMC 5% 1kN‡
Kc (Mpa.m1/2) 0.070 0.014 0.035 0.045 0.157 0.106 0.585 0.097 0.087 0.068
Gc (J/m2) 3.0 0.96 2.9 3.2 117.0 59.6 199.0 16.8 21.1 15.9
įc (m) 340 82.7 787 3510 641 703 1450 1360 1260 231
E (MPa) 567 191 261 465 266 441 1201 410 399 317
Gc/E (m) 5.29e-09 5.00e-09 1.10e-08 6.98e-09 4.39e-07 1.35e-07 4.10e-08 5.28e-08 5.02e-08
† DuPont corn herbicides ‡ 50 m glass beads with polymer binder
5.2.3. Empirical Crush Strength and Attrition Tests There are a plethora of ‘standard’ empirical tests for measuring granule strength or attrition resistance. The details of these are industry, or even company specific. They fall into two broad categories:
Crush strength tests Tests which measure size distribution after handling
Crush strength tests measure the fracture strength of individual granules or beds of granules under uniaxial compression. Although a compressive stress is applied, granules generally fail in tension via crack propogation. During compaction of single particles or beds of particles, particles break in quasistatic compression. For a single particle, the extent of breakage will relate to the fracture toughness of the particles. For beds of particles, the transmission of stress through the bed is complex. The first inflection on the compaction curve for a granular bed in uniaxial compression, the consolidation starting stress Pc , has been related to the crushing strength of individual particles by several workers (Couroyer et al., 1998; Naito et al., 1998; Adams and McKeown, 1996; Mort et al., 1995). Figure 5.10 shows an example of a compaction curve for spray dried alumina granules. However, compaction curves for granules that show brittle fracture are similar to those for plastic deformation so it is difficult a priori to extract granule mechanical properties from bed compaction tests. Most authors also compare bed compaction results to single granule crush strength, itself not a true property for brittle and semi-brittle fracture.
Figure 5.10. Typical compaction curve for spray dried alumina. ıyield indicates the onset of either plastic deformation or fracture of granules (Mort et al., 1995)
Handling tests measure the size distribution of granules (typically the % “fines”) after a specific type of handling. Various handling methods are used, including drop tests, fluidised beds, pneumatic conveying loops, tumbling or sieving with metal balls and rotation in a shear cell. It is important to realise that the mode of breakage in these empirical tests varies depending on the type of test (see section 5.2.4 below). These different modes of breakage have different functional dependence of fundamental material properties (fracture toughness, hardness) and flaw distribution. For this reason, breakage by one mode cannot be accurately predicted by a test base on a different breakage mode. In the worst case, different materials can rank differently in different tests, making even qualitative comparisons difficult. When empirical tests must be used, they should be chosen to mimic as closely as possible the expected handling conditions for the product in question. 5.2.4. Breakage Mechanisms for Dry Granules The process zone plays a large role in determining the mechanism of granule breakage. Agglomerates with small process zones in comparison to granule size break by a brittle fracture mechanism into smaller fragments (figure 5.11a). This mechanism is called fragmentation or fracture. However, for fracture to occur the granule must be able to concentrate enough elastic energy to propogate gross fracture during collision. This is harder to do as the process zone size increases. For well defined compacts under controlled stress testing conditions, it can
BREAKAGE AND ATTRITION
be shown both theoretically and experimentally that fracture will only occur when the specimen size is significantly larger than the process zone size (Kendall, 1978; Puttick, 1980). For many agglomerate materials, the process zone size is of the order of the granule size (see Table 5.1). These granules will break by wear, erosion or attrition brought about by diffuse microcracking (figure 5.11b). In contrast to fragmentation, these microcracking based processes lead to the generation of substantial amounts of fines. Thus, this class of breakage process is unfortunately both the most common and the most problematic.
Figure 5.11. Schematic of breakage by (a) fracture, and (b) erosion/attrition depending on process zone size
There is relatively little good quality data relating attrition/erosion rates of granules and agglomerates to fundamental properties. However, we can make use of knowledge developed in the ceramics and tribology literature, as well as breakage of single particles. The mode of stress application effects both the attrition rate and the functional dependence on particle properties. There are three classes of stress application: (i) wear and erosion, (ii) impact and (iii) compaction. For abrasive wear of agglomerates, the volumetric wear rate is (Evans and Wiltshire, 1976): V =
d11 / 2 A1 / 4 K c3 / 4 H 1 / 2
P 5 / 4l
where dI is indentor diameter, P is applied load, l is wear displacement of the indentor and A is apparent area of contact of the indentor with the surface. Note that the wear (erosion) rate is inversely dependent on both the fracture toughness and the hardness.
Experimental studies of the impact breakage of single crystals give a different dependence on material properties (Ghadiri et al. 1991; Yuregir et al 1987): V∝
ρ pu 2d p H K c2
Impact attrition is more sensitive to fracture toughness than abrasive wear. In addition the effect of hardness is the opposite to that for wear, since hardness acts to concentrate stress for fracture during impact. During compaction of single particles or beds of particles, particles break in quasistatic compression (section 5.2.3). Clear relationships with granule properties are not available but breakage rate will depend on fraction toughness (Kc), plasticity (Gc/E) and flaw distribution. Different modes of breakage will dominate in various processing equipment and attrition tests, and there is a different dependence on agglomerate properties for the three modes of breakage. These differences emphasises the need for fundamental properties to be known in order to estimate attrition rates by different processes. 5.2.5. Case Study – Fluid Bed Attrition of Agglomerates Within a fluid bed there are a large number of low velocity collisions between particles as they shear past each other. This process is analogous to abrasive wear. The number and relative velocity of the collisions depends on the number of bubbles in the bed and hence the excess gas velocity (U-Umf). The applied pressure in a fluid bed depends on bed depth. Thus by analogy to the wear process described by eqn.5-8, we can write: Bw =
d 01 / 2 K c3 / 4 H 1 / 2
hb5 / 4 (U − U mf )
where hb is the fluidised bed height and do is the distributor hole orifice size. We will now test the effect of granule properties on the attrition rate. The materials shown in Table 5.1 were formed into bars and their wear rate against a rough surface measured (Ennis and Sunshine, 1993). Results are shown in figure 5.12a. The dependence on fracture toughness and hardness matches that predicted by eqn. 5-10. Figure 5.12b shows the attrition rate of granules of these materials in a fluid bed. The relationship between attrition rate and agglomerate properties is remarkably similar. This confirms that wear is a key mechanism of fines production in fluid beds and that the relative attrition rate can be accurately predicted if some fundamental mechanical properties of the agglomerate material are known.
BREAKAGE AND ATTRITION
5.3. Particle Design for Controlling Attrition and Breakage Table 5.2 summarises typical changes in formulation and operating variables which can be used to minimise granule attrition and breakage. Granule attrition will increase with decreasing macroscopic fracture toughness, increasing flaw size and increasing intensity in handling. Figure 5.13 illustrates the point. The attrition rate for several formulations is a strong function of the granule density (porosity). The effect of porosity on macroscopic properties is two-fold. Firstly, macroscopic fracture toughness increases with decreasing porosity due to the increased number of bonds per unit volume and the increased strength of the bonds. Secondly, the maximum flaw size increases with porosity. However, even at the same porosity, there are very significant differences between the attrition resistance of different formulations. No amount of granule densification can completely overcome poor bonding between the particles. Attrition resistance can be improved by a combined effort in formulation design and process choice. 5.3.1. Effect of Process Variables For granulation processes without simultaneous drying the effect of process intensity is quite clear. Granule attrition resistance is increased with increasing process intensity because the granule porosity is decreased (see chapter 4). Increasing residence time in the granulator may also decrease the granule porosity if the resistance of the wet granule to densification is large. For granulators with simultaneous drying, the picture is much cloudier. Both wet and dry granules exist in the granulator. Increasing process intensity will both increase the density of wet granules (decreasing attrition) and increase the rate of attrition of dry granules in the granulator. Modifying bed temperature, spray rate or spray drop size to increase the drying (consolidation) time may be a more rewarding alternative in this case. Note that the range of porosities that can be achieved for any one granulator is quite limited. Major changes to porosity (and strength) may require more intense processes such as high shear mixers or compaction processes.
(b) Figure 5.12. Erosion rates of agglomerate materials (a) during wear test on formed bars; (b) attrition of granules in a fluidised bed
BREAKAGE AND ATTRITION
Figure 5.13. Effect of granule porosity on fluidised bed attrition of five agricultural chemical formulations
5.3.2. Effect of Formulation Properties Both granule fracture toughness and hardness are strongly influenced by the compatibility of the binder with the primary particles and the elastic/plastic properties of the binder. If the binder has poor compatibility with the particles, adhesive failure will occur with the bond between the binder and the particle breaking. With high compatibility binders, cohesive failure (within the bond) may be the failure mechanism (figure 5.14). In principle, macroscopic granule properties can be derived from knowledge of the microscopic adhesive and cohesive failure modes. The microscopic fracture toughness of a bond between particles can be measured by nanoindentation techniques. Where polymeric binders are used, the adhesion between polymer and a surface similar to the particle can be measured by a peel test. Feed powder size will also influence macroscopic properties. In general, reducing particle size increases attrition resistance as (a) the number of bonds per unit volume is increased, and (b) the size of pores (flaws) is smaller. Fine powder granules are more difficult to compact, however, so that the precise effect of feed powder size is very dependent on the consolidation processes in the granulation.
Figure 5.14. Cohesive failure in the Klucel bridge between glass spheres within a granule
BREAKAGE AND ATTRITION
Table 5.2. Controlling Breakage in Granulation Processes Typical changes in material or operating variables which minimize breakage
Appropriate routes to alter variable through formulation changes
Increase fracture toughness Maximize overall bond strength Minimize agglomerate voidage
Increase binder concentration or change binder. Bond strength strongly influenced by formulation and compatibility of binder with primary particles.
Increase hardness to reduce wear Minimize binder plasticity Minimize agglomerate voidage
Increase binder concentration or change binder. Binder plasticity strongly influenced by binder type. Change binder. Binder plasticity strongly influenced by binder type. Apply coating to alter surface hardness. Lower-formulation density.
Decrease hardness to reduce fragmentation Maximize binder plasticity Maximize agglomerate voidate Decrease load to reduce wear
Decrease contact displacement to reduce wear
Decrease impact velocity to reduce fragmentation
Appropriate routes to alter variable through process changes
Decrease binder viscosity to increase agglomerate consolidation by altering process temperatures (usually decrease for systems with simultaneous drying). Increase bed-agitation intensity (e.g., increase impeller speed, increase bed height) to increase agglomerate consolidation. Increase granulation-residence time to increase agglomerate consolidation, but minimize drying time. See above effects which decrease agglomerate voidage.
Reverse the above effects to increase agglomerate voidage.
Decrease bed-agitation and compaction forces (e.g., mixer impeller speed, fluid-bed height, bed weight, fluid-bed excess gas velocity, drum rotation speed). Decrease contacting by lowering mixing and collision frequency (eg., mixer impeller speed, fluid-bed excess gas velocity, drum rotation speed). Decrease bed-agitation intensity (e.g., mixer impeller speed, fluid-bed excess gas velocity, drum rotation speed). Also strongly influenced by distributor-plate design in fluid-beds, or impeller and chopper design in mixers.
5.3.3. Controlling Granule Dispersibility In some applications, the end use of granules requires them to be redispersed in water. In this case, granule need to be easily wetted (chapter 3). Once wet, granules need to rupture quickly under as additives in the formulation such as clays expand when wet. Clearly the wetting properties of the granule are important, but also the energy required to rupture the granule under internal stress Gc (eqn 5.6). Figure 5.15 shows (1) increasing granule porosity improves dispersibility, and (2) the ranking of formulations for dispersibility is almost the reverse of their ranking for attrition resistance (figure 5.13). Achieving a good
ce between granule handling properties and their redispersion properties is tricky. In this respect, the role of wetting and swelling agents in the formulation of water dispersible granules is very important to achieve fast dispersing granules that still maintain reasonable dry attrition resistance for handling.
5.4. Concluding Comments We are still “scratching the surface” in our understanding of the fundamentals of granule breakage. Further research work is needed and the key is understanding the fracture mechanics of both wet and dry granules. Nevertheless, we can still use our limited understanding for particle design and process scale up as has been shown by several examples in this chapter. Beware of empirical attrition tests. Use results from these tests with great care and try to match the test to the expected handling conditions for the granules.
Figure 5.15. Dispersibility of five agricultural chemical formulations – effect of granule porosity
5.5. Bibliography Adams, M.J. and Briscoe, B.J. (1987). Tribology in Particulate Technology, Adam Hilger, Bristol, England. Adams, M.J. and McKeown, R. (1998). Powder Technology, 88 (2), 155. Coureyer, C., Ning, Z., Bassam, M. and Gahadiri, M. (1998). Proc. 3rd World Congress on Particle Technology, Brighton, UK, IChemE, Paper No.61. Dencs, B. and Ormos, Z. (1993). Hung J Ind. Chem., 21 (3), 225.
BREAKAGE AND ATTRITION
Ennis, B.J. and Sunshine, G. (1993). Tribology International., 26, 319 (1993). Evans, A.G. and Wilshaw, T.R. (1976). Acta Metall., 24, 939. Ghadiri, M., Yuregir, K.R., Pollock, H.M., Ross, J.D.J., Rolfe, N. (1991). Powder Technology, 65, 311-320. Holm, P., Jungerson, O., Schaefer, T. and Kristensen, H.G. (1983). Pharm. Ind. 45 (8), 806. Irwin, G.R. (1957). Trans. ASME: J. Appl. Mech., 24, 361. Johnsson, L. and Ennis, B.J. (1994). Proc.1st International Particle technology Forum, AIChE, Denver, 178-183. Kendall, K. (1978). Nature, 272, 710. Keningley, S.T., Knight, P.C., and Marson, A.D. (1997). Powder Technol., 91, 95. Knight, P.C., Johansen, A., Kristensen, Schaefer, T. and Seville, J.P.K. (2000). Powder Technol., 110, 209. Lawn, B.R. (1975). Fracture of brittle solids (2nd ed.), Cambridge Univ. Press, Cambridge. Mort, P.R. and Tardos, G.I. (1999). Kona, 17, 64. Naito, M., Nakahira, K., Hotta, T., Ito, A., Yokoyama, T. and Kamiya, H. (1998). Powder Technology, 95, 214 . Pearson, J.M.K., Hounslow, M.J., Instone, T. and Knight, P.C. (1998). Proc. 3rd World Congress on Particle Technology3, paper 86. Puttick, K. E. (1980). J. Phys. D: Apply. Phys., 13, 2249. Ramaker J. S., Jelgersma, M. A., Vonk P. and Kossen N.W.F. (1998). Inter. J. of Pharm.,166 (1), 89. Sastry, K.V.S. and Feurstenau, D.W. (1975). Int. J. Miner. Process, 2, 187. Tardos, G.I., Irfan-Khan, M. and Mort, P.R. (1997). Powder Technol., 94, 245. Khan M.I. and Tardos G.I (1997). J Fluid Mech., 347, 347. Vonk P., Guillaume C. P. F., Ramaker J. S., Vromans, H. and Kossen, N.W.F. (1997). Int. J. Pharm., 157, 93. Watano, S., Sato, Y., Miyanami, K. and Murakami, T. (1995). Chem. Pharm. Bull., 43(7) 1212. Yuregir, K.R., Ghadiri, M. and Clift, M. (1987). Chem. Eng. Sci., 42, 843.
5.6. Nomenclature A Bw C d0 dp dI d32 E H hb Kc l
indenter contact area (m2) attrition rate (kg s-1) crack length (m) orifice diameter (m) particle diameter (m) indenter diameter (m) Sauter mean size of particles (m) Young’s modulus (Pa) hardness (Pa) fluid bed height (m) Fracture toughness (Pa.m1/2) wear displacement of indenter (m)
ied load (N) rp particle radius (m) * critical Stokes deformation number (-) St def
Stokes deformation number (-)
Stokes viscous number (-)
u U Umf V Y ȡp Ĳ Ĳy
impact velocity (m s-1) fluidization velocity (m s-1) minimum fluidization velocity (m s-1) volumetric attrition rate (m3 s-1) geometric factor (-) particle density (kg m-3) shear stress (Pa) yield stress (Pa)
CHAPTER 6 MATHEMATICAL MODELLING OF AGGLOMERATION PROCESSES Figure 1.5 showed that a granulator can be analysed in several scales. So far, we have analysed important granulation rate processes at the particle and volume-of-powder scale (chapters 3 to 5). In this chapter, we describe the balance equations that describe the evolution of granule property distributions in the granulator ie. granulator scale analysis. A key tool in this analysis is the population balance. The population balance (PB) is a rate equation which follows the change in number of particles of a given property(ies). The equation is analogous to the mass balance (continuity) equation for a chemical species which is familiar to chemical engineers. It includes convective (flow) terms, accumulation and a kinetic expression for each mechanism which changes the particle property similar to chemical reaction kinetics in reactor design (see figure 6.1). By combining the PB with overall mass and energy balances and information on mixing patterns in the granulator, we can apply traditional process engineering analysis to the granulation unit operation. The population balance was introduced as a general equation for particulate systems independently by Hulbert and Katz (1964) and Randolph and Larsen (1962). It is a powerful tool with uses including: • • • •
critical evaluation of data to determine controlling mechanisms in design, to predict the mean size and size distribution of product particles sensitivity analysis: to analyse quantitatively the effect of changes in operating conditions or feed variables on product quality optimisation and process control
Despite its power, the equation has been little used outside academic circles for attacking granulation problems. This contrasts markedly to crystallisation and grinding, where the population balance is a widely used design tool. There are two key historical reasons for this: • •
the usefulness of the models is very dependent on knowledge of the kinetic parameters. These have been difficult to predict for granulation systems. solution to the equations is difficult, especially for coalescence problems.
These historical problems are now largely overcome so that the population balance has come of age as a tool for engineers and technologists dealing with granulation processes. In this chapter the population balance is derived, starting from the definitions of property distributions discussed in chapter 2. Rate expressions for the important granulation processes are developed and the rate parameters related to the quantitative understanding developed in chapters 3 to 5. Analytical and numerical solution techniques are briefly described and application case studies are presented 143
THE SCIENCE AND ENGINEERING OF GRANULATION
Q flow rate:
x fI ,xf2' x fJ " ,
T, P.. .. . flow rate:
X"" x ,,2' X p3 '"
T, P.... .
flow rate: size dist": properties:
n,,, nf2 , nf3 '" Pp'Y"_al,, ,etc.
Iprod~ flow rate:
size dist" : npl ,n,,2 ,np3 '" properties: